Gallium Nitride -based Microwave Power Varactors for Wireless Base Station Applicationsкод для вставкиСкачать
UNIVERSITY OF CALIFORNIA, SAN DIEGO GaN-based Microwave Power Varactors for Wireless Base Station Applications A dissertation submitted in partial satisfaction of the requirements for the degree Doctor of Philosophy in Electrical Engineering (Applied Physics) by Wei Lu Committee in charge: Professor Paul K.L. Yu, Chair Professor Peter M. Asbeck, Co-Chair Professor Prabhakar R. Bandaru Professor Andrew C. Kummel Professor Yu-Hwa Lo 2013 UMI Number: 3557816 All rights reserved INFORMATION TO ALL USERS The quality of this reproduction is dependent upon the quality of the copy submitted. In the unlikely event that the author did not send a complete manuscript and there are missing pages, these will be noted. Also, if material had to be removed, a note will indicate the deletion. UMI 3557816 Published by ProQuest LLC (2013). Copyright in the Dissertation held by the Author. Microform Edition © ProQuest LLC. All rights reserved. This work is protected against unauthorized copying under Title 17, United States Code ProQuest LLC. 789 East Eisenhower Parkway P.O. Box 1346 Ann Arbor, MI 48106 - 1346 Copyright © Wei Lu, 2013 All rights reserved. The Dissertation of Wei Lu is approved, and it is acceptable in quality and form for publication on microfilm and electronically: _____________________________________________________________________ _____________________________________________________________________ _____________________________________________________________________ _____________________________________________________________________ Co-Chair _____________________________________________________________________ Chair University of California, San Diego 2013 iii DEDICATION To my beloved wife Wen Qiao. iv EPIGRAPH There are no secrets to success. It is the result of preparation, hard work, and learning from failure. Colin Powell v TABLE OF CONTENTS Signature Page ……………………………………………………………………… iii Dedication …………………………………………………………………………... iv Epigaph ……………………………………………………………………………… v Table of Contents …………………………………………………………………… vi List of Figures ………………………………………………………………………..ix List of Tables …………………………………………………………………….... xvi Acknowledgments ..…………………………………………………………….… xvii Vita …………………………………………………………………………………xxii Abstract of the Dissertation ...…………………………………………………..…xxiv Chapter 1 Introduction ........................................................................................... 1 1.1 Introduction to varactors.................................................................................... 1 1.2 Figure of merit for GaN-based microwave power varactors ............................. 3 1.3 Overview of the dissertation .............................................................................. 7 1.4 References ....................................................................................................... 10 Chapter 2 Design of GaN-based microwave power varactors ............................ 11 2.1 Design for high breakdown voltage ................................................................ 11 2.2 Design for high linearity .................................................................................. 19 2.3 Design for high Q ............................................................................................ 20 2.4 Summary of the designs .................................................................................. 24 2.5 References ....................................................................................................... 25 Chapter 3 Ni-InGaN/GaN Schottky diode technology ...................................... 27 vi 3.1 Theory of InGaN surface layer design ............................................................ 28 3.1.1 Analysis of reverse leakage current in GaN Schottky barriers ................. 28 3.1.2 InGaN surface layer design for reduced leakage current ......................... 34 3.2 Experimental results and discussions .............................................................. 38 3.2.1 C-V measurements and analysis ............................................................... 38 3.2.2 Forward I-V measurements and analysis ................................................. 40 3.2.3 Reverse I-V measurements and analysis .................................................. 44 3.3 Leakage current reduction using higher pressure GaN buffer ......................... 48 3.4 InGaN/GaN material growth and characterization .......................................... 52 3.4.1 InGaN/GaN MOCVD growth .................................................................. 53 3.4.2 InGaN/GaN material characterization ...................................................... 56 126.96.36.199 Reported defects in GaN and InGaN materials ................................. 57 188.8.131.52 Experimental procedures ................................................................... 59 184.108.40.206 X-ray diffraction measurements ........................................................ 60 220.127.116.11 Nomarski microscope imaging .......................................................... 61 18.104.22.168 Surface topography investigation by SEM and AFM ....................... 62 22.214.171.124 Etch pit density measurements .......................................................... 64 126.96.36.199 Discussion of material defect characterization .................................. 67 3.4.3 Electrical characteristics of InGaN/GaN Schottky diodes ....................... 70 3.4.4 Effects of thermal annealing on Ni-InGaN/GaN Schottky diodes ........... 75 3.5 Application for enhancement-mode HFETs .................................................... 78 3.6 Summary of InGaN/GaN technology .............................................................. 83 3.7 Reference ......................................................................................................... 85 Chapter 4 Fabrication procedure ........................................................................ 91 4.1 Introduction ..................................................................................................... 91 4.2 Initial fabrication procedure ............................................................................ 92 4.3 Preliminary results ........................................................................................... 96 vii 4.3.1 I-V measurements ..................................................................................... 96 4.3.2 RF measurements ..................................................................................... 98 4.4 Sidewall passivation in GaN-based Schottky diodes .................................... 107 4.4.1 Simulation of electric field distribution under reverse biases ................ 107 4.4.2 Experimental procedure.......................................................................... 112 4.4.3 Results and discussions .......................................................................... 114 4.4.4 Summary of sidewall passivation in GaN-based Schottky diodes ......... 117 4.5 Improved fabrication procedure .................................................................... 117 4.6 Summary of the fabrication procedure .......................................................... 119 4.7 References ..................................................................................................... 121 Chapter 5 5.1 Experimental results and discussions .............................................. 122 High voltage I-V and C-V measurements ..................................................... 122 5.2 S-parameter measurements ............................................................................ 125 5.2.1 Measurements for the 1-port devices ..................................................... 128 5.2.2 Measurements for the 2-port devices ..................................................... 136 5.3 Linearity measurements................................................................................. 146 5.3.1 Two-tone test .......................................................................................... 146 5.3.2 2-W WCDMA signal input .................................................................... 150 5.4 Application in the tunable resonant circuit .................................................... 152 5.5 Summary........................................................................................................ 155 Chapter 6 Conclusion and Future Work........................................................... 157 6.1 Summary of the thesis ................................................................................... 157 6.2 Comparison of different varactor technologies ............................................. 160 6.3 Future work ................................................................................................... 162 6.4 References ..................................................................................................... 164 Appendix A GaN-based varactor fabrication procedure ........................................ 165 viii LIST OF FIGURES Figure 1-1 Schematic structure of Schottky-diode based semiconductor varactor.…………...….......................... …...…...…...…...…..... 4 Schematic diagram of a GaN-based varactor and its layer structure.……..... …….....…….....…….....…….....……............ 12 Figure 2-2 SEM top view of a fabricated diode with an 80-μm diameter…. 13 Figure 2-3 Reverse leakage current of a device with an area of 5 × 10−5 cm2.......………….....………….....………….....………….....… 14 Schematic diagram of the GaN-based Schottky diode design with thin InGaN surface layer for breakdown voltage enhancement.…………………………………………..… …… 16 (a) Schematic diagrams of the (upper) electric field and energy bands under the same reverse bias for the designs with InGaN/GaN and GaN only. (b) Representative energy band diagrams at reverse 0 and 100 V calculated by the 1-D Poisson solver.…....... ….......….......….......….......….......….......…........ 16 Reverse IV characteristics for samples with and without InGaN surface layers. Circular diodes have areas of 5×10−5 cm2……... 18 Simulated CV curves for (a) single diode structure and (b) two anti-parallel diode structure.………..…….… ..……. ..……….. 20 Schematic diagram of the anti-parallel diode structure with interdigitated strip geometry.………….….……………. ….….. 21 (a) Schematic diagram of the anti-parallel varactor diode with its corresponding lump components, and (b) the circuit model represented by a distributed resistance and capacitance……….. 22 Figure 2-10 Simulated values of Q as a function of finger length....……...... 23 Figure 3-1 Schematic energy band diagram of a Schottky barrier under reverse bias.………………... ………...………...………...…… 33 Figure 2-1 Figure 2-4 Figure 2-5 Figure 2-6 Figure 2-7 Figure 2-8 Figure 2-9 Figure 3-2 Experimental and calculated reverse leakage current of a Ni- ix Figure 3-3 Figure 3-4 Figure 3-5 Figure 3-6 Figure 3-7 Figure 3-8 Figure 3-9 Figure 3-10 Figure 3-11 Figure 3-12 Figure 3-13 Figure 3-14 GaN Schottky diode with an area of 5×10-5 cm2.……………… 34 (a) Schematic diagram of the electric field under the same reverse bias for the designs with InGaN/GaN, GaN/InGaN/GaN and GaN only. (b) Representative energy band diagrams (Ec only) at Vr = 0V and (c) Vr = 80 V by solving the 1-D Poisson equation.……………………………... 37 C-V results of the five samples with area of 7.85×10-5 cm2, measured in the dark at 1 MHz. The colored dots are measurement data and the dash lines are fitting curves………... 39 Schematic energy band diagram of an InGaN/GaN Schottky barrier under forward bias.………………….............................. 42 Forward I-V curves of the five samples with areas of 5×10-5 cm2.…..............………..............………..............………............ 43 Currents at reverse bias 50 V as a function of diode area for the control and 0nm/In0.06Ga0.94N samples.……………………....... 45 Reverse I-V curves of the five samples with area of 5×10-5 cm2.………………………………………………...................... 47 The histogram of the breakdown voltages for the control and InGaN-containing diodes..………………………....................... 48 Reverse I-V curves of the samples using HP and LP GaN buffer layers with area of 5×10-5 cm2………………………….. 50 Forward I-V curves of the Control_HP and 2nm/In0.1Ga0.9N_HP samples with area of 5×10-5 cm2................ 52 The histogram of SBHs extracted from the experimental forward I-V curves of the Control and Control_HP samples...... 52 Thomas Swan close-coupled showerhead (CCS) 3×2’’ MOCVD system..……………………........................................ 54 The indium percentage and FWHMs of (0002) X-ray rocking curve (XRC) of thick InGaN films for different growth temperatures and molar flow ratios of TMIn/(TMIn+TMGa) during growth………………………………………………….. 55 x Figure 3-15 a) Schematic cross section of the InGaN/GaN Schottky diode and (b) the Nomarski optical microscopy top view of a real diode with surface micromesas.……………………………… 59 Nomarski optical microscopy images of (a) HP_InGaN/GaN, (b) LP_InGaN/GaN, (c) HP_GaN and (d) LP_GaN.…………... 62 Representative SEM and AFM (tapping mode) micrographs of the surface micromesas.………………………………………... 63 10 × 10 m2 AFM images of (a) HP_InGaN/GaN, (b) surface profile along the line in (a), (c) LP_InGaN/GaN, and (d) surface profile along the line in (c) after H3PO4 etch.…………. 64 Figure 3-19 Surface micromesa mapping by Nomarski optical microscopy.. 66 Figure 3-20 An AFM (tapping mode) micrograph of surface micromesas with and without nanopipes at the center……………………… 69 Leakage current at a reverse bias of 30 V versus diode diameter for LP_InGaN/GaN and HP_InGaN/GaN Schottky diodes…………………………………………………………... 71 Leakage current at a reverse bias of 30 V versus micromesa number on the smallest (17-m diameter) LP_InGaN/GaN and HP_InGaN/GaN Schottky diodes……………………………… 73 Representative forward IV curves for the smallest (17-m diameter) Ni-InGaN/GaN Schottky barriers (a) without surface micromesas and (b) with surface micromesas…………………. 73 Representative reverse-bias IV curves for the smallest (17-m diameter) Ni-InGaN/GaN Schottky barriers (a) without surface micromesas and (b) with surface micromesas…………………. 75 RBS spectra of as-deposited, annealed at 200 oC for 60 minutes, 500 oC for 24 minutes and 625 oC for 15 minutes NiInGaN/GaN samples…………………………………………… 76 Leakage current at a reverse bias of 30 V versus diode diameter for LP_InGaN/GaN and HP_InGaN/GaN Schottky diodes before and after annealing at different temperatures…… 78 Figure 3-16 Figure 3-17 Figure 3-18 Figure 3-21 Figure 3-22 Figure 3-23 Figure 3-24 Figure 3-25 Figure 3-26 xi Figure 3-27 Simulated AlGaN/GaN and InGaN/AlGaN/GaN HEMT structures and the corresponding energy band diagrams………. 80 Simulated I-V characteristics for AlGaN/GaN and InGaN/AlGaN/GaN HEMTs…………………………………... 82 Schematic diagram of the anti-parallel diode structure with interdigitated strip geometry.………........................................... 92 Schematic diagrams of the initial GaN-based varactor fabrication procedure……………….………………………….. 95 Reverse leakage current tracking after critical fabrication steps. (a) Before and after sputtering SiNx and (b) before and after BCB curing……………………….……………………………. 97 Figure 4-4 Measurement setup for S11.……………….…………………... 98 Figure 4-5 S11 measured from a device at reverse bias of 40 V from 50 MHz to 5.05 GHz shown in a Smith Chart.…………….……… 100 Figure 4-6 Q factor versus frequency at a reverse external bias of 40 V for an anti-parallel varactor diode.…………………..…………….. 100 Figure 4-7 Reverse I-V characteristics of an anti-parallel varactor diode… Figure 4-8 Equivalent circuit model for the anti-parallel varactors with considering Rleak for the reverse leakage current……….……… 102 Figure 4-9 Extracted series resistance (a) and Q (b) versus reverse external biases for 1GHz, 2GHz and 3GHz……….……………………. 103 Figure 4-10 Relations between series resistance and Rleak, and series capacitance and Rleak.…………………………………………... 104 Figure 4-11 Experimental and simulated C-V curves for one of the diode in the two back-to-back diodes…………………….……………... 104 Figure 4-12 (a) Experimental Q (dots) and simulated Q (lines) versus the reverse external bias at f = 1 GHz, 2 GHz and 3 GHz; (b) experimental Q (dots) and simulated Q (at reverse external biases of 20 V, 40 V and 60 V) versus frequency….………….. 106 Figure 3-28 Figure 4-1 Figure 4-2 Figure 4-3 xii 101 Figure 4-13 Simulated Q versus reverse biases assuming the reverse leakage is low at high biases.………………………….……….. 106 Figure 4-14 Simulated GaN Schottky diode structure with sidewall passivation in Silvaco ATLAS 2-D simulator for electric field distribution under reverse biases..…...………………………… 109 Figure 4-15 Sidewall passivation by (a) growing dielectrics along the sidewall and (b) Mg+ implantation through the sidewall……… 109 Figure 4-16 (a) Electric field distribution under a reverse bias of 85 V and (b) peak electric field at the edge of Ni-GaN Schottky junctions for different passivation materials along the GaN sidewalls……………………………………………………….. 110 Figure 4-17 Electric field distribution for a device with a non-self-aligned gate process…………………………………………………….. 111 Figure 4-18 Fabrication procedure for sidewall passivation by Mg+ implantation……………………………………………………. 114 Figure 4-19 Reverse leakage current for samples fabricated with different sidewall processing procedures. The diode area is 2.8×10-5 cm2……………………………………………………………... 116 Figure 4-20 Improved fabrication procedure and the resultant reverse I-V characteristics………………………………………………….. 119 Figure 5-1 Forward I-V characteristics for a 60-m-diameter circular diode in the sample.……….………………………….………... 123 Figure 5-2 Reverse I-V characteristics for a 60-m-diameter circular diode in the sample.……………………………………………. 123 Figure 5-3 (a) High voltage C-V characteristics for a circular diode with an area of 5×10-5 cm2 at f = 1 MHz and (b) the corresponding tuning ratio vs RF peak-to-peak voltage for the anti-parallel diode varactor, based on the considerations of not causing reverse breakdown or forward conduction.………………......... 125 Figure 5-4 (a) An optical microscopy image of a device for 1-port measurements, (b) an optical microscopy image of a device for 2-port measurements, (c) the equivalent series LRC network for the 1-port device and (d) the equivalent series LRC xiii network for the 2-port device.………………………….……… 127 Figure 5-5 Reverse I-V curve for a 1-port anti-parallel diode varactor. The dots are the measurement data points.…………...…………….. 129 Figure 5-6 S11 from 500 MHz to 3.5 GHz for a 1-port device at a reverse bias of 70 V.……………………………………..……………... 129 Figure 5-7 The relations of (a) Q versus reverse bias, (b) Rs versus reverse bias and (c) Cs versus reverse bias at 1 GHz, 2 GHz and 3 GHz for a 1-port device….…………………………………………... 131 Figure 5-8 The relation of Q versus frequency at different reverse biases for a 1-port device........................................................................ 132 Figure 5-9 Equivalent circuit model considering the parasitics from the 1port device and the measurement setup.…….............................. 133 Figure 5-10 Experimental and simulated Q versus frequency curves at different reverse biases for a 1-port device. …………………... 135 Figure 5-11 Schematic diagram for the 2-port measurements.……............... 136 Figure 5-12 Reverse I-V curve for a 2-port anti-parallel diode varactor. The dots are the measurement data points.………............................. 137 Figure 5-13 The representative S-parameters for the varactor 2-port measurements………………………………………………….. 138 Figure 5-14 The relations of (a) Q versus reverse bias, (b) Rs versus reverse bias and (c) Cs versus reverse bias at 1 GHz, 2 GHz and 3 GHz for a 2-port device………………………………………... 140 Figure 5-15 The experimental and simulated Cs versus reverse bias curves for a 1-port device……………………………………………… 141 Figure 5-16 The relation between Q and frequency at different reverse biases for a 2-port device………………………………………. 142 Figure 5-17 Experimental and simulated Q versus frequency curves at different reverse biases for a 2-port device……………………. 143 Figure 5-18 Optical microscopy images and the corresponding experimental Q versus frequency curves for the 2-port devices xiv with different areas and structures……………………………... 145 Figure 5-19 Measurement setup for the two-tone test………………………. 147 Figure 5-20 Output power at fundamental and IM3 frequencies versus the input power for an anti-parallel diode varactor (1-port) at a control reverse bias of 25 V……………………………………. 148 Figure 5-21 Measurement setup for the WCDMA signal input experiment... 150 Figure 5-22 Adjacent channel leakage ratio (ACLR) for a small 1-port device with a 2-W (12-W peak power) WCDMA signal input... 151 Figure 5-23 (a) Equivalent circuit model of the measurement system for the WCDMA signal input experiment, and (b) simulated instantaneous RF voltage at different nodes…………………… 152 Figure 5-24 Measurement setup of the tunable resonant circuit using the varactor and transmission lines………………………………… 153 Figure 5-25 (a), (b) Experimental and (c), (d) the corresponding simulated S21 curves from 0.5 GHz to 2.5 GHz, for the tunable resonant circuit using varactor and transmission lines…………………... 154 xv LIST OF TABLES Table 1-1 Comparison of properties and varactor figure of merit for various semiconductors.…………... ……………………….… 7 Table 2-1 Sample layer structures and labels.... ………………………… 17 Table 3-1 Sample labels and key growth details used in this study..……. 35 Table 3-2 Values of the parameters used for all calculations (including forward and reverse I-V curves) in this work.…… …….……. 44 Table 3-3 Sample labels and key growth details used in this work.…….. 60 Table 3-4 FWHM of symmetric (0002) and asymmetric (10-12) XRCs, surface micromesa density estimated under Nomarski optical microscopy and nanopipe and TD densities estimated by EPD in all samples.……………. …………………………………… 61 Samples treated with different sidewall cleaning and passivation methods.………………………... ... ... ... ... ... ... ... 115 Measured and simulated OIP3 for the anti-parallel diode varactor with different n factors.….….………………………... 149 The performance parameters of different varactor technologies. ….….……….….……….….……….….……….. 161 Table 4-1 Table 5-1 Table 6-1 xvi ACKNOWLEDGEMENTS First of all, I would like to thank my dissertation advisor, Professor Paul Yu, who provided enlightening guidance and tremendous support throughout my research and life in the last six years at UCSD. He brought me to the world of MOCVD and Gallium Nitride, in which I found my interests. I am deeply indebted to my co-advisor, Professor Peter Asbeck, whose incisive and insightful advices always led me to the right directions. I am most impressed by his solid and comprehensive knowledge as well as his great patience during his discussions with students. I would like to acknowledge Professor S. S. Lau, who was my teacher of ECE 136L and offered me a TAship for ECE 136L later on. He is not only my teacher of academics but also a good mentor of personality. I am very grateful to Prof. Tohru Nakamura, who is a professor in Hosei University. He provided lots of valuable comments to my thesis research and co-authored several papers during his visit at UCSD. I would like to thank Prof. Yu-Hwa Lo, who was my teacher of ECE 230A and ECE 236B as well as my thesis committee member. Also I am grateful for his excellent guidance to my wife’s thesis research. I would like to thank Prof. Prabhakar R. Bandaru and Prof. Andrew C. Kummel for serving as my thesis committee members. I would like to express my special thanks to my previous advisor Professor Yan Huimin at Zhejiang University, who always advise me selflessly not only in the xvii research but also in my life. I would like to thank many other professors who taught me in classes and offered me all kinds of help at UCSD, including Prof. Yuan Taur, Prof. Jie Xiang, Prof. Deli Wang, Prof. Zhaowei Liu, Prof. Gabriel M. Rebeiz, etc. I am most thankful for Mr. David Aplin and Arthur Clawson for their work training and helping me to keep the MOCVDs running smoothly and very thorough and practical discussions on crystal growth. I would like to thank Dr. Lingquan (Dennis) Wang for his great guidance and help on several projects and paper writing. He is not only my good friend but also a good teacher of mine. I would like to thank Dr. Winnie Chen for her excellent training skills to help me become an experimental researcher. I would also like to thank those who were labmates and great coworkers, including Dr. Xiaobo Xie, Dr. Justin Bickford, Jeff Bloch, Dr. Meredith Draa, Dingbo Chen, Siyuan Gu, Hayg Dabag, Johana Yan, Dr. Paul Theilmann, Kangmu Lee, Wenyi Rai, Daniel Estrada, Conway Wang and Jianzhi Wu. Many thanks to friends and collaborators, including Dr. Peng Chen, Dr. Arthur Zhang, Dr. Hua Li, DanYong Lu, Feifei Wei, Muchuan Yang, Ke Sun, Yi Jing, Yuchun Zhou, Yanjin Kuang, and many of whom graciously lent me their time and lab equipment. I would like to acknowledge the staffs at Nano3, Dr. Bernd Fruhberger, Larry Grissom, Ryan Anderson, Xuekun Lu, Sean Parks, Ahmet Erten, and Dr. Maribel xviii Montero for their help in the cleanroom whenever needed. I would also like to thank all of the staffs at ECE, especially Cheryle Wills, Shana Slebioda, etc. My deepest thanks go to my family. I am grateful to my parents whose selfless love and sacrifice are always the power for success. I am so indebted to my wife who is a great source of intelligence in our family and encourages me all the time when I encountered difficulties. All of the achievements I made she has a share. I owe lots of care to my son at his early ages. To all my family, I owe the greatest thanks for being the indispensable support of my growth. Finally I would like to acknowledge the financial sponsors of my Ph.D research projects, including the FutureWei Technologies Inc., the University of California at San Diego Center for Wireless Communications, the National Science Foundation grant of NSF-ECCS-901113, the National Science Foundation under the program NIRT0506902, the UC Discovery Grant Program, the Army Research Office sponsored DURIP and the Department of Energy under the EERE-PMC program DEFG36-08GO18016. Section 1.1, 2.2 and 2.3, are a rearrangement of the project proposal “High Power Varactor Development for Adaptive Basestations,” Peter M. Asbeck. The dissertation author was the primary researcher of this project. xix Section 1.2 and 2.1, are a rearrangement of the paper “InGaN/GaN Schottky Diodes With Enhanced Voltage Handling Capability for Varactor Applications,” Wei Lu, Lingquan Wang, Siyuan Gu, David P. R. Aplin, Daniel M. Estrada, Paul K. L. Yu, and Peter M. Asbeck, IEEE Electron Device Letters, vol. 31, no. 10, pp. 1119–1121, Oct. 2010. The dissertation author was the primary author of the paper. Section 3.1, 3.2 and 3.3, are a rearrangement of the paper “Analysis of Reverse Leakage Current and Breakdown Voltage in GaN and InGaN/GaN Schottky Barriers,” Wei Lu, Lingquan Wang, Siyuan Gu, David P. R. Aplin, Daniel M. Estrada, Paul K. L. Yu, and Peter M. Asbeck, IEEE Trans. Electron Devices, vol. 58, no. 7, pp. 1986– 1994, Jul. 2011. The dissertation author was the primary author of the paper. Section 3.4, is a rearrangement of the paper “Effects of surface micromesas on reverse leakage current in InGaN/GaN Schottky barriers,” Wei Lu, Tomoaki Nishimura, Lingquan Wang, Tohru Nakamura, Paul K. L. Yu, and Peter M. Asbeck, J. Appl. Phys., vol. 112, pp.044505, Aug. 2012. The dissertation author was the primary author of the paper. Section 4.3, is a rearrangement of the paper “InGaN/GaN Microwave Varactors with High Q, High-Breakdown Voltage and High Linearity,” Wei Lu, Lingquan (Dennis) Wang, Siyuan Gu, David P. R. Aplin, Paul K. L. Yu, and Peter M. Asbeck, in Semiconductor Device Research Symposium (ISDRS), 2011 International, xx IEEE, College Park, MD, 7-9 Dec., 2011. The dissertation author was the primary author of the paper. xxi VITA 2005 B. S., Optical and Electrical Engineering Zhejiang University, Hangzhou, China 2007 Completion of Graduate Study, Optical Engineering Zhejiang University, Hangzhou, China 2011 M. S., Electrical Engineering (Applied Physics) University of California, San Diego, USA 2013 Ph. D., Electrical Engineering (Applied Physics) University of California, San Diego, USA PUBLICATIONS W. Lu, L. Wang, S. Gu, D. P. R. Aplin, D. M. Estrada, P. K. L. Yu, and P. M. Asbeck, “InGaN/GaN Schottky Diodes with Enhanced Voltage Handling Capability for Varactor Applications,” IEEE Electron Device Lett., vol. 31, no. 10, pp. 1119–1121, Oct. 2010. W. Lu, L. Wang, S. Gu, D. P. R. Aplin, D. M. Estrada, P. K. L. Yu, and P. M. Asbeck, “Analysis of Reverse Leakage Current and Breakdown Voltage in GaN and InGaN/GaN Schottky Barriers,” IEEE Trans. Electron Devices, vol. 58, no. 7, pp. 1986–1994, Jul. 2011. W. Lu, L. Wang, S. Gu, D. P. R. Aplin, P. K. L. Yu, and P. M. Asbeck, “InGaN/GaN Microwave Varactors with High Q, High-breakdown Voltage and High Linearity,” in Semiconductor Device Research Symposium (ISDRS), 2011 International, IEEE, College Park, MD, 7-9 Dec., 2011. W. Lu, T. Nishimura, L. Wang, T. Nakamura, P. K. L. Yu, and P. M. Asbeck, “Effects of Surface Micromesas on Reverse Leakage Current in InGaN/GaN Schottky Barriers,” J. Appl. Phys., vol. 112, pp.044505, Aug. 2012. S. Gu, H. Katayose, K. Nomoto, T. Nakamura, A. Ohoka, K. Lee, W. Lu, and P. xxii M. Asbeck, “High Transconductance Ion-Implanted GaN MISFETs Using Atomic Layer Deposited High-k Dielectrics,” Phys. Status Solidi C, 2013. W. Lu, L. Wang, S. Gu, P. M. Asbeck, and P. K. L. Yu, “Critical Design Considerations for GaN-based Microwave Power Varactors,” in Electronic Devices and Solid State Circuits (EDSSC), 2012 International, IEEE, Bangkok, Thailand, 3-5 Dec., 2012. W. Lu, D. Aplin, A. R. Clawson, and P. K. L. Yu, “Effects of the Gas Ambient in Thermal Activation of Mg-doped p-GaN on Hall Effect and Photoluminescence,” Journal of Vacuum Science and Technology A, vol. 31, 011502, Jan. 2013. FIELD OF STUDY Major Field: Electrical Engineering Focused Field: Applied Physics xxiii ABSTRACT OF THE DISSERTATION GaN-based Microwave Power Varactors for Wireless Base Station Applications by Wei Lu Doctor of Philosophy in Electrical Engineering (Applied Physics) University of California, San Diego, 2013 Professor Paul K. L. Yu, Chair Professor Peter M. Asbeck, Co-Chair With the development of wireless communication systems, the demand for providing tunability in the wireless communication circuits becomes more and more intense. Among the technologies, semiconductor varactor is the critical component that is capable of implementing tunable and adaptive characteristics, particularly for the frond-end components of the wireless communication systems. For base station applications, high voltage handling capability, typically of 100 V or greater, high xxiv quality factor (Q), typically of above 100 at operation frequency, and high linearity, OIP3 > 65 dBm, are required. This work will mainly discuss in detail the design, fabrication and characterization to achieve the high-voltage high-Q and high-linearity microwave power varactors for wireless base station applications. Some preliminary varactor applications in the test tunable circuits will be demonstrated too. In this dissertation, we first introduce the physics of the semiconductor varactors and the motivation for choosing GaN as the candidate material for this microwave power varactor. Then we elucidate the critical design considerations for achieving high breakdown voltage, high quality factor and high linearity. The novel Schottky barrier engineered design using a thin InGaN surface layer on top of GaN to enhance the breakdown voltage of GaN-based Schottky diodes is therefore introduced. We then show the theoretical and experimental studies on the suppression mechanisms for electron tunneling in the InGaN/GaN Schottky barriers. The detailed material characterization for the InGaN/GaN material system and its application for the enhancement-mode HEMTs are also presented. Next, we discuss the initial device fabrication procedure and the improving methods based on the initial DC and RF measurement results. Thereafter, we report the detailed characterizations of the fabricated devices including the high-voltage I-V and C-V, S-parameters for 1-port and 2-port devices, linearity and application in the tunable resonant circuits. Finally, we summarize the dissertation and outline the future work. In this work, we achieved a high-performance GaN-based microwave power varactors with breakdown voltage > 100 V, quality factor > 100 and OIP3 > 71 dBm. It meets the initial goal of this project as well as the specifications in some practical xxv applications. To the best of our knowledge, this combination of breakdown voltage, Q and OIP3 represents remarkable advancement from any other reported varactors. xxvi Chapter 1 Introduction 1.1 Introduction to varactors Future generations of wireless base station systems need to respond to a wide variety of requirements concerning carrier frequency, output power, modulation bandwidth and peak-to-average ratio. To meet these requirements, the base stations need to be much more adaptive than they are at present. It is envisioned that the carrier frequency should be able to be controllably varied over a wide spectral range, to make use of different channels and different bands. The characteristics of the amplifiers should also be controllably variable in order to adapt to different environments and different specifications, such as output power level, antenna condition, and linearity specifications. Such adaptation requirements can provide new levels of performance to base stations utilizing the architecture currently in use; and even greater benefits can be obtained with future architectures based on software defined radio concepts, where a single RF front-end, under software control, can meet the requirements for all bands and signaling formats. Cognitive radio is a further development of this idea, in which "white spaces" in the RF spectrum are identified and utilized for opportunistic 1 2 transmissions. To permit this adaptability while maintaining satisfactory performance of high RX (receive) input sensitivity and high TX (transmit) output efficiency, very high performance tunable microwave filters and matching networks are required. In turn, new enabling components are needed in order to provide this tunability. One of the most promising avenues is to develop tunable capacitors (or varactors). For base station applications, however, the varactors must be able to handle very high voltage levels (peak RF voltages above 100 V), have very high Q (greater than 100), and have very high linearity. This combination of specifications has not been obtainable to date with available technologies - which include semiconductor varactors, MEMS, and ferroelectric-/piezoelectric- based  systems. The key objective of this research is to develop varactor diodes capable of providing high Q in high power operation and to demonstrate them in adaptive microwave circuits. Comparing with MEMS, or ferroelectric-/piezoelectric-based varactor technology, semiconductor Schottky diode varactors provide faster tuning and higher reliability. Semiconductor varactors have traditionally been implemented with Si or GaAs-based diodes, for which the depletion region thickness (depletion capacitance) can be varied with applied voltage. The resultant devices, however, typically do not have sufficient voltage handling capability for the output of a power amplifier, or, if they are designed particularly for high voltage operation, then their Q values at microwave frequencies are too low, so that they cause significant loss of output power and efficiency. The linearity of the varactors is also a critical concern. SiC power varactors have been recently developed and reported . This research 3 explores varactors based on GaN materials, which have dramatic new opportunities for improved performance in high-power microwave applications; the relevant figure of merit (see next section) for GaN is 40× larger than that of Si for this application. The new varactors are an enabling technology for wireless base stations, since for the first time, the varactors will be able to operate at the power levels required in the base station front-ends. 1.2 Figure of merit for GaN-based microwave power varactors Microwave varactors provide the ability to tune the impedance matching of microwave components, and varying the operating frequency of amplifiers, oscillators and filters. They are important elements for the implementation of tunable and adaptive microwave systems and can assist in enabling efficient multi-band and software-defined radios. Critical considerations for the application of microwave varactors are: the maximum to minimum capacitance ratio (r), the maximum voltage handling capability (Vmax), and the microwave loss (as represented by the Q value, defined below). In order to apply varactors to the tuning of microwave power amplifiers, it is typically necessary to have large capacitance ratios (r>2~3), high voltage handling capability (Vmax >25V and up to 200V), and high Q values (Q>200). The proposed study is based on our observation that GaN has significant material 4 advantages for the implementation of varactor diodes. A figure-of-merit is derived below, and shown to be larger for GaN than for Si by a factor of more than 40. A schematic diagram of a Schottky-diode based varactor is shown in Fig. 1. Under external bias control, the width of the depletion region is varied in the nvaractor region. Underlying this region, an n+ layer serves to provide contact to the backside. The Q value of the varactor under a given operating condition is the ratio of capacitive reactance to series resistance, and can be calculated by 1/(2fRC), where C is the capacitance, and R is the resistance at the operating condition (when the overall impedance is considered as a simple series RC network). Both R and C vary as the depletion capacitance is changed with the control voltage. The worst case Q is Qmin, which occurs generally when C reaches its maximum value. We will consider Qmin in the following. Figure 1-1 Schematic structure of Schottky-diode based semiconductor varactor. 5 For the varactor, the capacitance C is given by A/W, where W is the depletion region width at a given voltage bias, A is the junction area and is the dielectric constant of the semiconductor. Thus Cmax=A/Wmin (which occurs at the lowest control voltages), Cmin=A/Wmax (ignoring stray capacitances), and r=Wmax/Wmin. We will assume in the following that the doping level is constant in the lightly doped nvaractor region. The series resistance R comprises various contributions. In the following we neglect series resistance from contacts and n+ region, and assume that the undepleted portion of the "lightly doped" varactor region dominates the resistance. The width of this undepleted region (and hence the resistance) varies with the control voltage. R is then given by (Wmax-W)/A, where is the n- material resistivity, constant across the varactor region. Therefore, ( ) ( ) Eq. 1-1 The resistivity in the undepleted varactor region, , is given by 1/(nq), where n is the carrier density, the carrier mobility and q the charge of the electron. The carrier density (and the corresponding doping density Nd) is limited by the need to keep the maximum electric field, Emax, below the critical breakdown electric field, Ebk, when the varactor region is fully depleted. Using the constant Nd (constant n) design, this constraint is given by 6 Eq. 1-2 The maximum voltage supported under these conditions is Vmax= EmaxWmax/2. It follows that Nd <Ebk2/(2qVmax), and from the above it follows that [ ( ) ] Eq. 1-3 The factor Ebk2 constitutes a material figure of merit that indicates the potential of a given material for attaining high Q varactors, while the factor 1/[4(r-1)fVmax] corresponds to varactor design parameters, independent of material. The equation illustrates that attaining high Q is particularly challenging for circuits in which the voltage level is high (as needed in high power amplifiers). It is of interest to compare the varactor figure-of-merit for different semiconductor material technologies. Table 1-1 below shows values appropriate to Si, GaAs, InP and GaN . Values of Qmin are also calculated for a representative scenario (f=1 GHz, r=3, Vmax=100 V). The figureof-merit obtained for GaN is the highest in the table, higher than that of Si by a factor of more than 40×. This suggests that for microwave power amplifiers, designs based on GaN will be attractive. 7 Table 1-1 Comparison of properties and varactor figure of merit for various semiconductors. The calculated Qmin is shown for the materials for the condition f=1 GHz, r=3 and Vmax=100 V. Properties and Qmin Si GaAs InP GaN (cm /Vsec) 1200 4000 3500 500 Ebk (MV/cm) 0.25 0.35 0.40 2.5 12 Ebk (10 V/sec) 75 490 560 3125 Qmin 30 195 223 1240 2 2 Table 1-1 provides an upper bound to the Qmin that can be expected for a given material. In actual implementation, the series resistance will incorporate also portions corresponding to the n+ regions, bond-wires and interconnects, and potentially from the ohmic contact regions. 1.3 Overview of the dissertation This dissertation explores a technology to achieve high-voltage, high-Q and high-linearity microwave varactors in order to provide tunable and adaptive characteristics to the wireless base station systems. GaN with its high electron mobility and high breakdown electric field is used as the candidate material for this technology. In Chapter 1, the needs of microwave power varactors in the wireless base station applications are illustrated. The criteria for choosing the candidate semiconductor materials are also discussed. Chapter 2 details the design 8 considerations for achieving high breakdown voltage, high Q and high linearity. Epitaxial layer structure is designed to achieve the required breakdown voltage and Q. Optimized interdigitated and anti-parallel-diode device structures are used to improve the Q and linearity, respectively. Chapter 3 describes the invention of thin InGaN surface layer on top of GaN to enhance the Schottky barrier height and increase the breakdown voltage of the GaN-based Schottky diodes. InGaN/GaN material MOCVD growth, material characterization, thermal effects on Ni-InGaN/GaN Schottky junctions and its application in the enhancement-mode HEMTs are also presented. Chapter 4 discusses the fabrication procedure and preliminary DC and RF results of the microwave power varactors. Simulated and experimental results for various sidewall passivation methods to reduce reverse leakage current and maintain low leakage current during device fabrication are also reported. Chapter 5 demonstrates the final experimental DC and RF results and the corresponding simulations of the GaNbase microwave power varactors. Varactors with breakdown voltage of > 100 V, Q > 100 and OIP3 > 71 dBm (ACLR < -53 dBc) are achieved. Demonstration of the real application for the GaN-based microwave power varactors are also carried out by using the varactors in a tunable resonance circuit. Finally, Chapter 6 summarizes the entire dissertation and outlines the future work. Section 1.1, is part of the project proposal “High Power Varactor Development for Adaptive Basestations”, Peter M. Asbeck. The dissertation author was the primary researcher of this project. 9 Section 1.2, is part of the paper “InGaN/GaN Schottky Diodes With Enhanced Voltage Handling Capability for Varactor Applications”, Wei Lu, Lingquan Wang, Siyuan Gu, David P. R. Aplin, Daniel M. Estrada, Paul K. L. Yu, and Peter M. Asbeck, IEEE Electron Device Letters, vol. 31, no. 10, pp. 1119–1121, Oct. 2010. The dissertation author was the primary author of the paper. 10 1.4 References  P. Padmini, T. R. Taylor, M. J. Lefevre, A.S. Nagra, R. A. York and J. S. Speck, "Realization of high tunability barium strontium titanate thin films by RF magnetron sputtering," Applied Physics Letters, vol. 75, issue 20, pp. 3186-3188, Nov. 1999.  C. M. Andersson, N. Ejebjörk, A. Henry, S. Andersson, E. Janzén, H. Zirath, and N. Rorsman, "A SiC varactor with large effective tuning range for microwave power applications," IEEE Electron Device Lett., vol. 32, no. 6, pp. 788–790, Jun. 2011.  S. M. Sze and K. K. Ng, Physics of Semiconductor Devices, 3rd Edition. Hoboken, NJ: Wiley, 2007. Chapter 2 Design of GaN-based microwave power varactors GaN-based varactors have been previously reported mainly fabricated with a GaN HFET process -. In this chapter, we discuss the design of the GaN varactors with vertical geometry as shown before in Figure 1-1 and illustrate that a higher voltage handling capability may be obtained with a suitable InGaN surface layer design. Designs and simulations for optimizing the device layout to achieve high Q and high linearity will be also presented. 2.1 Design for high breakdown voltage Figure 2-1 schematically shows the structure of a GaN varactor with vertical geometry. In order to achieve a breakdown voltage of larger than 100 V, the varactor region (n- GaN) thickness is designed to be t = 2Vmax/Ebk = 1 m, where Vmax = 100 V 11 12 and Ebk is conservatively assumed to be 2 MV/cm. The doping concentration of the nGaN is estimated from 1-D Poisson equation: Nd = Ebk/(qt) = 1×1017 cm-3. The thickness and doping level of the underlying n+ GaN region should be thick and high enough, but without deteriorating the material quality, to minimize the series resistance coming from this layer. In this design, they are chosen to be ~1.5 m and 5×1018 cm-3, respectively. The material is grown on c-Sapphire substrates using metal organic chemical vapor deposition (MOCVD). Ni is used as the Schottky contact to ensure a high Schottky barrier height and Ti/Au/Pd/Au (Au is atop) metal stack is used as the ohmic contact. Figure 2-1 Schematic diagram of a GaN-based varactor and its layer structure. Then devices are fabricated and measured to verify the breakdown characteristics of the designed GaN Schottky diodes. The fabrication procedure is as follows: a 120-nm-thick Ni Schottky contact was deposited immediately after the sample MOCVD growth and NH4OH surface cleaning to minimize the interface 13 oxidation or contamination . The Ni film was then patterned, and circular mesa diodes with diameters in the range of 80–300 μm were formed using BCl3/Cl2 in a Trion reactive-ion-etching/inductively-coupled plasma dry-etch system, which was followed by an ∼90 oC KOH (0.1 mol/L) treatment to reduce the dry-etch residuals. A Ti/Al/Pd/Au (20 nm/80 nm/50 nm/100 nm) metal stack was used to form ohmic contacts to n+ GaN. A scanning-electron microscopy (SEM) top view of the fabricated device is shown in Figure 2-2. Figure 2-2 SEM top view of a fabricated diode with an 80-μm diameter. The current-voltage (I-V) characteristics of these diodes were measured with an Agilent B1500 semiconductor device analyzer. The reverse I-V curve of a diode with an area of 5×10−5 cm2 is shown in Figure 2-3. However, the breakdown voltage is lower and the reverse leakage current is higher than the expected values. The leakage 14 current under a high reverse bias has been attributed to the direct tunneling of electrons through the Schottky barrier , . For a proper operation and low-power loss of the GaN varactors, the leakage current of the Schottky diode must be adequately low even at high operating voltages. Therefore an improved design is needed to suppress the electron tunneling. Figure 2-3 Reverse leakage current of a device with an area of 5 × 10−5 cm2. It is known that large polarization-charge densities present at III–nitride semiconductor heterojunction interfaces significantly affect the electric-field distributions in the semiconductors , providing opportunities for Schottky-barrier engineering. To suppress the tunneling current under a high reverse bias, we designed an InGaN surface layer to engineer the tunneling barrier by utilizing the polarization charges at the InGaN/GaN interface. The new design and its corresponding electric field and energy band diagrams are shown in Figure 2-4 and 2-5, respectively. As 15 shown in Figure 2-5(a), in comparison to the design with GaN only, the surface electric field is reduced for the InGaN surface layer design, which leads to an increased electron tunneling distance. The significant reduction (∼50% at a 100-V reverse bias) of the surface electric field is primarily due to the presence of the negative polarization charges at the InGaN/GaN interface, although the slightly increased dielectric constant of the InGaN also favors the surface field reduction. The suppression of the leakage current is thus achieved because the tunneling probability sharply decreases with the increase of the tunneling distance. The indium concentration and the thickness of the InGaN layer are designed to be 10% and 15 nm, respectively, based on the considerations of obtaining high-quality InGaN layers and resultant energy barrier shape. Figure 2-5(b) shows the corresponding energy band diagram at reverse 0 and 100 V by solving a 1-D Poisson equation. In this computation, a 4.9 × 1012 cm−2 sheet polarization charge density and a 0.21-eV conduction band energy discontinuity  at the In0.1Ga0.9N/GaN interface were assumed. The Schottky barrier height of In0.1Ga0.9N was also assumed to be 0.21 eV lower than that of the GaN. As seen, at reverse 100 V, the tunneling distance for the InGaN/GaN design is ∼2 times larger than the design with GaN only. 16 Figure 2-4 Schematic diagram of the GaN-based Schottky diode design with thin InGaN surface layer for breakdown voltage enhancement. Figure 2-5 (a) Schematic diagrams of the (upper) electric field and energy bands under the same reverse bias for the designs with InGaN/GaN and GaN only. W and W’: Depletion width. L and L’: Electron tunneling distance. Δξ: Surface electric field reduction. (b) Representative energy band diagrams at reverse 0 and 100 V calculated by the 1-D Poisson solver . 17 The samples with and without InGaN surface layer design were grown using a Thomas Swan Close Coupled Showerhead 3×2 MOCVD system. For comparison purposes, three samples have been grown, with layer information and labels shown in Table 2-1. The Schottky diodes were then fabricated followed the same procedure stated above. The measured reverse IV characteristics are shown in Figure 2-6. Table 2-1 Sample layer structures and labels. Sample labels Control In0.06Ga0.94N In0.1Ga0.9N InGaN layer N.A. 6 % indium, ~15 nm 10 % indium, ~15 nm n- GaN (n~1×1017 cm-3, 1 m) Common n+ GaN (n~5×1018 cm-3, 1.5 m) layers undoped GaN buffer (~1.5 m) c-sapphire substrate 18 Figure 2-6 Reverse IV characteristics for samples with and without InGaN surface layers. Circular diodes have areas of 5×10−5 cm2. It is obvious that the inclusion of the InGaN surface layer significantly improves the breakdown voltage by up to ∼40 V, in comparison with the control sample. Such improvement is consistently observed, for all of our InGaN-containing samples, as a result of the reduced surface electric field, as shown in Figure 2-5(a). These results validated the approach of implementing a thin InGaN surface layer on top of GaN is effective in achieving the GaN-based high-voltage microwave varactors. The detailed analysis including forward and reverse I-V, capacitance-voltage (C-V), material and thermal characteristics of the Ni-InGaN/GaN Schottky diodes will be discussed chapter 3. 19 2.2 Design for high linearity In order to maintain adequate linearity in the amplifier, the effective varactor capacitance should not vary with the RF signal level. However, a single Schottky diode varactor has poor linearity due to the square root dependence of the capacitance on the applied voltage: C~V-1/2, for a uniformly doped junction. A well-established strategy to improve the linearity of diode-based varactors is to employ an anti-parallel (back-to-back) diode topology , in the geometry shown in Figure 2-7(b). In this circuit, the DC control voltage is applied to both diodes equally. The RF voltage swing, however, adds to the instantaneous voltage of each diode with opposite sign (such that the capacitance of one of the diodes is increased, while the other is decreased). The net capacitance under the application of DC voltage and RF voltage can be readily calculated; representative results for both two diode topologies are shown in Figure 2-7 for simple diodes with uniform n- doping. It is seen that by using the anti-parallel diode topology, the RF signal induced capacitance variation is minimized. The linearity of the varactor diode is thus significantly improved. An optimal choice of semiconductor doping profile can improve linearity further . 20 Figure 2-7 Simulated C-V curves for (a) single diode structure and (b) two antiparallel diode structure. In this design, a center resistor, also called “control resistor” is needed to maintain a high Q factor. The impedance of the control resistor should be high enough to prevent the loss of the RF signal through the DC path (maintaining high Q factor), but not cause too much voltage drop through the DC path (maintaining tuning characteristics). In our design, the resistance of the control resistor Rctrl is typically > 10×│1/jC│, where is the operation frequency and C is the capacitance of the antiparallel varactor. More design considerations on improving the Q will be discussed in the following section. 2.3 Design for high Q 21 In order to achieve high Q, the series resistance of the structure needs to be minimized. The component of resistance associated with the undepleted n- region is decreased by doping the n- region as high as is feasible, as discussed in section 1.2. The component of resistance associated with the n+ backside contact is decreased by increasing the doping and thickness of the n+ layer, and by decreasing the separation of the varactor regions. As a result of these considerations, an interdigitated stripe geometry is adopted, as shown schematically in Figure 2-8. The dimensions of the stripes are made as small as possible, consistent with the lithography and etch techniques available. The serpentine resistor made by n+ GaN is the control resistor for blocking RF signals in the DC path. The design constraint of the Rctrl is described in the previous section. Figure 2-8 Schematic diagram interdigitated strip geometry. of the anti-parallel diode structure with 22 The series resistance expected from the n+ regions under the diodes is the principal parasitic; by contrast, the resistance from the undepleted n- GaN region is usually very small. Bondwires add additional series resistance, exacerbated by skin effect as the frequency increases. An additional concern of significance for Q is the series resistance of the stripe (interdigitated) Schottky metal contacts. The distributed resistance of these metals can add appreciably to the overall resistance if the fingers are too long. In order to find out the optimal geometry of the interdigitated structure for the purpose of achieving high Q, a transmission line method considering the corresponding lump components is used to estimate the overall contribution from different regions of the structure. Fig. 2-9(a) shows the schematic diagram of an interdigitated diode structure with its corresponding lump components. The transmission-line circuit model was represented by a distributed resistance and capacitance as shown in Figure 2-9(b). Figure 2-9 (a) Schematic diagram of the anti-parallel varactor diode with its corresponding lump components, and (b) the circuit model represented by a distributed resistance and capacitance. 23 The calculation result shows that the overall Q is a function of finger length, with maximum values that differed according to the metal sheet resistance used, as detailed in Figure 2-10. A maximum Q value is achieved for a finger length of ~ 50 m under the assumption of 2.5-m finger width and spacing and 1-m metal stripe thickness. Too long or too short metal length will result in a lower Q. 160 140 R =0.15 s R =0.10 s R =0.05 s Q @ 1GHz 120 100 80 60 40 20 Figure 2-10 25 30 35 40 45 Finger Length (um) 50 55 60 Simulated values of Q as a function of finger length. Another lump component that is not considered in this model is the Rleak in parallel with the series Rn- and Cd, which represents the leakage path of the Schottky barrier. A small value of Rleak (corresponding to a leaky junction) will cause an increase of the series resistance so that the Q drops. The detailed analysis of reverse leakage current will be discussed in chapter 4. 24 2.4 Summary of the designs This chapter covered the designs for achieving high-breakdown voltage, highQ and high-linearity GaN-based microwave Schottky varactor diodes. A thin InGaN surface layer design is invented to increase breakdown voltage of the GaN-based Schottky diodes by ~40 V, from ~80 V to above 120 V. The anti-parallel diode topology will be adopted to improve the linearity performance of varactors. Interdigitated structure with small and optimized finger dimensions (upon the lithograph and processing techniques) and thick metal stripe will be used to maximize the Q. Section 2.1, is a rearrangement of the paper “InGaN/GaN Schottky Diodes With Enhanced Voltage Handling Capability for Varactor Applications”, Wei Lu, Lingquan Wang, Siyuan Gu, David P. R. Aplin, Daniel M. Estrada, Paul K. L. Yu, and Peter M. Asbeck, IEEE Electron Device Letters, vol. 31, no. 10, pp. 1119–1121, Oct. 2010. The dissertation author was the primary author of the paper. Section 2.2 and 2.3, are a rearrangement of the project proposal “High Power Varactor Development for Adaptive Basestations”, Peter M. Asbeck. The dissertation author was the primary researcher of this project. 25 2.5 References  M. Saglam, K. Mutamba, A. Megej, C. Sydlo, H. L. Hartnagel, and I. Daumiller, “Influence of polarization charges in Al0.4Ga0.6N/GaN barrier varactors,” Appl. Phys. Lett., vol. 82, no. 2, pp. 227–229, Jan. 2003.  C. S. Chu, Y. G. Zhou, K. J. Chen, and K. M. Lau, “Q-factor characterization of RF GaN-based metal-semiconductor-metal planar interdigitated varactor,” IEEE Electron Device Lett., vol. 26, no. 7, pp. 432–434, Jul. 2005.  M. Marso, A. Fox, G. Heidelberger, P. Kordos, and H. Luth, “Comparison of AlGaN/GaN MSM varactor diodes based on HFET and MOSHFET layer structures,” IEEE Electron Device Lett., vol. 27, no. 12, pp. 945–947, Dec. 2006.  I. J. Lee, C. Yu, H. J. Shin, J. Y. Kim, Y. P. Lee, T. B. Hur, and H. K. Kim, “ Oxidation study of polycrystalline InN film using in situ X-ray scattering and X-ray photoemission spectroscopy,” Thin Solid Films, vol. 515, no. 11, pp. 4691–4695, Apr. 2006.  F. A. Padovani and R. Stratton, “Field and thermionic-field emission in Schottky barriers,” Solid State Electron., vol. 9, no. 7, pp. 695–707, Jul. 1966.  T. Hashizume, J. Kotani, and H. Hasegawa, “Leakage mechanism in GaN and AlGaN Schottky interfaces,” Appl. Phys. Lett., vol. 84, no. 24, pp. 4884–4886, Jun. 2004.  O. Ambacher, J. Majewski, C. Miskys, A. Link, M. Hermann, M. Eickhoff, M. Stutzmann, F. Bernardini, V. Fiorentini, V. Tilak, B. Schaff, and L. F. Eastman, “Pyroelectric properties of Al(In)GaN/GaN hetero- and quantum well structures,” J. Phys.: Condens. Matter, vol. 14, no. 13, pp. 3399–3434, Apr. 2002.  H. Zhang, E. J. Miller, E. T. Yu, C. Poblenz, and J. S. Speck, “Measurement of polarization charge and conduction-band offset at InxGa1−xN/GaN heterojunction interfaces,” Appl. Phys. Lett., vol. 84, no. 23, pp. 4644–4646, Jun. 2004.  Gregory Snider, “1-D Poisson solver,” http://www3.nd.edu/~gsnider/ 26  K. Buisman, L. C. N. de Vreede, L. E. Larson, M. Spirito, A. Akhnoukh, T. L. M. Scholtes, and L. K. Nanver, “Distortion-free varactor diode topologies for RF adaptivity,” in Proc. IEEE MTTS Int. Microwave Symp., Long Beach, CA, pp. 157–160, Jun. 2005. Chapter 3 Ni-InGaN/GaN Schottky diode technology III–nitride-based Schottky diodes have achieved many applications, such as ultraviolet photodetectors , gas sensors , high-voltage rectifiers , and varactors . One key factor to improve the performance of these devices is to minimize reverse leakage current, particularly under high reverse voltages. For microwave power varactors, excess leakage current can cause Q degradation, device heating and reliability issue. Many prior efforts have been reported to reduce the leakage current in GaN-based Schottky barriers, such as electrochemical surface treatment , SiO2 dielectric surface passivation , capping with low-temperature GaN layers , and oppositely doped surface layers to increase the Schottky-barrier height (SBH) . However, these studies do not discuss in detail the leakage-current-suppression mechanisms particularly under high reverse voltages, which is important in highpower applications. In this chapter, we present a detailed study of the reverse-leakagecurrent mechanisms in MOCVD-grown GaN Schottky barrier diodes as well as the leakage-suppression mechanism using InGaN/GaN Schottky barriers. We also report that the leakage current can be further significantly suppressed by using a high- 27 28 pressure (HP, near atmospheric pressure) MOCVD growth technique  for the GaN buffer layers (i.e., an HP GaN buffer). Additionally, extensive InGaN/GaN material characterization using Nomarski optical microscopy, scanning electron microscopy, and atomic force microscopy are performed to correlate between the material defects and the excess reverse leakage current in Ni-InGaN/GaN Schottky barrier diodes. The application of InGaN/GaN design in the enhancement-mode GaN-based high electron mobility transistors (HEMTs) is also introduced. 3.1 Theory of InGaN surface layer design Based on the introduction of the InGaN surface layer design for enhancing the breakdown voltages of the GaN-based Schottky diode varactors, furthermore analytical studies on the reverse leakage current and leakage current suppression mechanisms in the GaN-based Schottky diodes will be discussed in this section. 3.1.1 Analysis of reverse leakage current in GaN Schottky barriers The reverse leakage current of the Schottky barrier has been attributed to the electron tunneling directly through the Schottky barrier , . In order to suppress the leakage current, it is necessary to re-examine the leakage current mechanisms in 29 GaN Schottky barriers. Figure 3-1 shows a schematic energy band diagram of a Schottky barrier under reverse bias. According to conventional analysis , for reverse biases greater than 3kT/q the current density Jr from semiconductor to metal through the Schottky barrier can be expressed by the following: AT q exp b P( ) exp d k kT kT 0 AT q (Vb ) Fm P( )1 Fs (Vr )d 0 k JA JB Jr Eq. 3-1 where A* is the effective Richardson constant, T is the temperature in Kelvin, k is the Boltzmann constant, q is the charge of an electron, qb is the effective barrier height, Vb is the built-in potential at reverse bias Vr ignoring image force lowering, q is the image force lowering of the barrier height, Fm and Fs are the Fermi-Dirac distribution functions of electrons in the metal and semiconductor, respectively, and are the energy of the electrons above and below the top of the effective barrier, respectively, and P() and P() are the tunneling probabilities of the electrons above and below the top of the effective barrier, respectively. Assuming P() = 1 and P() calculations using the Wentzel-Kramers-Brillouin (WKB) approximation , we find 2m P( E ) exp 2 x2 x1 q ( x) E dx 30 Eq. 3-2 where m* is the electron effective mass, ћ is the reduced Planck constant, x is the distance measured from the metal-semiconductor interface, and x1 and x2 are the classical turning points, which determine the electron tunneling distance as L = x2 - x1. Measured from the Fermi level of metal, (x) is the electrostatic potential distribution and E = qb - is the energy of tunneling electrons. In Eq. 3-1, the first term JA corresponds to the thermionic emission component; the second term JB corresponds to the tunneling component which dominates at high dopings and low temperatures. Therefore, we need only to consider the second term for studying n- GaN Schottky barriers at room temperature. Under low reverse bias P(E) sharply decreases as E decreases based on Eq. 3-2; most of the electrons tunnel near the top of the effective barrier so that 1 – Fs ≈ 1, and Fm is given by Fm 1 E exp . E E fm kT 1 exp kT Eq. 3-3 Assuming the barrier has a triangular shape near the top of the effective barrier, the electrostatic potential distribution can be written as: 31 q ( x) qx qb0 Eq. 3-4 where is the constant electric field near the top of the effective barrier. Then, Eq. 3-2 becomes 2m P( E ) exp 2 qb 0 E q 0 qx qb 0 E dx 3 2 q E 4 2 m . b0 exp 3 q Eq. 3-5 Ignoring JA, Jr can be approximated as: 3 2 q E AT qb 0 4 2 m E b0 Jr JB exp dE. (Vr Vn ) k q kT 3 Eq. 3-6 Taking a derivative of the exponential factor in Eq. 3-6, we can find the energy Em where the electron tunneling peaks: 2 q 2 2 Em qb 0 2 2 . 8m k T Eq. 3-7 32 Assuming the semiconductor has a uniform doping concentration Nd, Eq. 3-7 becomes 2 q 3 N d (Vb 0 Vr ) Em qb 0 4m*k 2T 2 Eq. 3-8 where Vb0 is the built-in potential at zero bias, and is the dielectric constant of the semiconductor. Eq. 3-8 is a decreasing function with the reverse bias Vr and valid as long as Eq. 3-3 is a good approximation (Em > 3kT). With further increasing Vr, Em eventually becomes almost constant when it reaches a few kT below the Fermi level of metal where Fm is almost constant at 1 but P(E) decreases sharply as E decreases further. Therefore, under high reverse bias most of the electrons tunnel near the Fermi level of metal. For a Ni/n-GaN Schottky barrier with Nd = 1×1017 cm-3, T = 300 K, and qb0 = 1 eV, Em = 1 – 0.03 × (0.92 + Vr) in eV. When Vr > 33 V most of the electrons tunnel near the Fermi level of metal. This finding suggests that the leakage current suppression under high reverse bias can be achieved by reducing the electron tunneling probability around the Fermi level of metal. 33 Figure 3-1 Schematic energy band diagram of a Schottky barrier under reverse bias. qb0 is the barrier height ignoring image force lowering, q is the image force lowering of the barrier height, qb = qb0 - q is the effective barrier height, Efm is the Fermi level of metal, Ef is the quasi-Fermi level of semiconductor, Ec is the bottom of the conduction band of semiconductor, qVn = Ec - Ef, E is the energy of electrons measured from the Fermi level of metal, Em is a certain energy where the electron tunneling peaks, Vb is the built-in potential at reverse bias Vr ignoring image force lowering, x is the distance measured from the metal-semiconductor interface, and L = x2 – x1 is the tunneling distance at Em. Anticipating the measurement results reported below, we find that the theoretical analysis outlined above agrees well with our experimental measurements. Figure 3-2 shows the measured reverse leakage current for a control sample (Ni/nGaN Schottky diode with Nd ≈ 1×1017 cm-3 confirmed by C-V measurement) with an area of 5×10-5 cm2 and for comparison the calculated result based on Eq. 3-1 with Nd = 1.1×1017 cm-3, qb0 = 0.95 eV, T = 300 K, A* = 26.4 Acm-2K-2 , m* = 0.2m0 , where m0 is the electron mass. Departures from the tunneling based curve occur at low bias (< 30 V) are possibly related to generation of minority carriers at defects within the depletion region, and at high bias (> 80 V). For Vr = 80 V, the calculated electric field at the surface reaches = 1.9 MV/cm, where impact ionization effects are expected to become significant. 34 Figure 3-2 Experimental and calculated reverse leakage current of a Ni-GaN Schottky diode with an area of 5×10-5 cm2. 3.1.2 InGaN surface layer design for reduced leakage current Five samples have been grown using the conventional low-pressure (LP) MOCVD growth technique  for the study of InGaN surface layer design. Their labels and key growth details are shown in Table 3-1. The Schottky diodes were fabricated followed the procedure mentioned in section 2.1. 35 Table 3-1 Sample labels and key growth details used in this study. Sample Control labels GaN cap 2nm/In0.06Ga0.94N 0nm/In0.06Ga0.94N UID, ~2nm, 400 N.A. layer mbar, 820 oC 2nm/In0.1Ga0.9N 0nm/In0.1Ga0.9N UID, ~2nm, 400 N.A. mbar, 808 oC N.A. UID, ~6% In, ~15 UID, ~6% In, ~15 UID, ~10% In, UID, ~10% In, nm, 400 mbar, nm, 400 mbar, ~15 nm, 400 ~15 nm, 400 820 oC 820 oC mbar, 808 oC mbar, 808 oC InGaN N.A. layer n- GaN (n~1×1017 cm-3, 1 m), 200 mbar, 1040 oC n+ GaN (n~5×1018 cm-3, 1.5 m), 200 mbar, 1040 oC Common Unintentionally doped (UID) GaN buffer (~1.5 m), 300 mbar (900 mbar used for HP layers GaN buffer), 1040 oC Low-temperature GaN nucleation layer (~20 nm), 600 mbar, 530 oC c-Sapphire substrate Based on the analysis in the last section, an InGaN surface layer is introduced to reduce the electron tunneling probability around the Fermi level of metal by Schottky barrier engineering. As shown in Figure 3-3, the surface electric field is significantly reduced for the InGaN surface layer design (InGaN/GaN case) due to the polarization charge at the interface, leading to an increased electron tunneling distance near the Fermi level of metal where most of the electrons tunnel under high reverse bias as discussed above. The leakage current is thus suppressed because the tunneling probability P(E) given by Eq. 3-2 sharply decreases with the increase of the tunneling distance. In addition to the samples discussed in section 2.1, a 2-nm-thick GaN cap 36 layer was also designed (GaN/InGaN/GaN) in case there was indium out-diffusion during the cooling down process at the end of the MOCVD growth. The GaN cap could, however, weaken the effectiveness of the InGaN surface layers (less tunneling distance increase compared to that without GaN cap layer as shown in Figure 3-3(c)). In order to obtain high-quality InGaN layers and long tunneling distances, we designed the indium concentration and the thickness of the InGaN surface layer to be 10% and 15 nm, respectively. Higher indium concentration and thicker InGaN thickness might result in InGaN layer quality degradation and strain relaxation (less polarization effects). The corresponding energy band diagrams at 0 and reverse bias 80 V shown in Figure 3-3(b) and 3-3(c), respectively, were obtained by solving the 1-D Poisson equation. In this calculation, a 4.9×1012 cm-2 sheet polarization charge density and a 0.21-eV conduction band discontinuity were assumed at the In0.1Ga0.9N/GaN and GaN/In0.1Ga0.9N interfaces ; the SBH (ignoring the image force lowering) of In0.1Ga0.9N was also assumed to be 0.21 eV lower than that of the GaN, which corresponds with the expected conduction band energy difference Ec between the In0.1Ga0.9N and GaN. It is seen that the tunneling distance for the In0.1Ga0.9N/GaN design at reverse bias 80 V is nearly doubled compared to the GaN only design. 37 Figure 3-3 (a) Schematic diagram of the electric field under the same reverse bias for the designs with InGaN/GaN, GaN/InGaN/GaN and GaN only. Δξ is the surface electric field reduction of the InGaN/GaN design relative to GaN-only design. (b) Representative energy band diagrams (Ec only) at Vr = 0V and (c) Vr = 80 V by solving the 1-D Poisson equation. 38 3.2 Experimental results and discussions Characterization of the Schottky diodes was carried out with C-V and I-V measurements. 3.2.1 C-V measurements and analysis Capacitance measurements were carried out using 1 MHz signals. Figure 3-4 shows plots of 1/C2 versus reverse voltage V. Curves for different samples exhibit slight differences of slope due to small variations (< 1%) of the fabricated diode areas and the doping concentration Nd of the n- GaN layers, which is approximately 1×1017 cm-3 (assuming complete ionization) extracted from the C-V results. It is noted that the curves of the InGaN-containing samples consistently show a voltage shift when compared to the control sample. This shift is due to the change in electric field distribution and electrostatic potential in the InGaN layers caused by the induced polarization charges, as shown in Figure 3-3(a). The voltage shift can be estimated by considering the integral of the electric-field reduction between the GaN and the InGaN layers, which is over the width of the InGaN layer. This estimate results in the expression: V tq InGaN t 2 Nd q 2 InGaN Eq. 3-9 39 where V is the voltage shift, t is the InGaN layer thickness, is the sheet polarization charge density at the InGaN/GaN interface, and InGaN is the dielectric constant of InGaN. As shown in Figure 3-4, V are ~0.6 and ~0.8 V for In0.06Ga0.94N- and In0.1Ga0.9N-containing samples, respectively. Using Eq. 3-9, the polarization charge density at the In0.06Ga0.94N/GaN and In0.1Ga0.9N/GaN interfaces are estimated to be 1.9×1012 cm-2 and 2.7×1012 cm-2, respectively. The estimated numbers are less than theoretical expectations (0.9×1012 cm-2 and 4.0×1012 cm-2 for the spontaneous and piezoelectric polarizations, respectively, in the In0.06Ga0.94N/GaN samples, and 1.5×1012 cm-2 and 6.4×1012 cm-2 for the spontaneous and piezoelectric components, respectively, for In0.1Ga0.9N/GaN) ,  probably due to partial strain relaxation. Figure 3-4 C-V results of the five samples with area of 7.85×10-5 cm2, measured in the dark at 1 MHz. The colored dots are measurement data and the dash lines are fitting curves. 40 3.2.2 Forward I-V measurements and analysis The polarization charges at the InGaN/GaN interfaces change the Schottky barrier shape and correspondingly the forward I-V characteristics. Figure 3-5 illustrates schematically the energy band diagram of an InGaN/GaN structure. The effective barrier height qb is forward-bias (Vf) dependent and given by qb qb 0 q q Wd N d q t Ec InGaN Eq. 3-10 where Ec is the conduction band discontinuity at the InGaN/GaN interface and Wd is the forward-bias dependent depletion width measured from the InGaN/GaN interface. It may be calculated by Wd 2 GaN (b Vn V f ) Nd q Eq. 3-11 where GaN is the dielectric constant of GaN. With Eqs. 3-10 and 3-11 the following equation holds 41 b t GaN . V f t GaN Wd InGaN Eq. 3-12 Using the thermionic emission (TE) theory, the forward I-V characteristics may be described as qb qV f J f AT 2 exp exp kT kT qV qb 1 AT 2 exp f . kT Eq. 3-13 Therefore the ideality factor n (or inverse subthreshold slope) may be obtained as q log10 J f n 1 b V 2.3kT V f f 1 1 1 t GaN . Wd InGaN Eq. 3-14 As shown by Eq. 3-14, the ideality factors for the indium-containing samples are expected to be bias dependent and greater than unity. 42 Figure 3-5 Schematic energy band diagram of an InGaN/GaN Schottky barrier under forward bias. Efm is the Fermi level of metal, Ec is the conduction band discontinuity, is the sheet polarization charge density at the InGaN/GaN interface, qb0 is the barrier height ignoring image force lowering, qb is the effective barrier height, Vf is the forward bias, t is the InGaN thickness and Wd is the forward bias dependent depletion thickness measured from the InGaN/GaN interface. Figure 3-6 shows the experimental I-V curves of the control and In0.06Ga0.94Ncontaining samples and the correspondingly theoretical calculations in the semilogarithmic scale. The ideality factors are 1.08 for the control sample, and 1.33 and 1.30 for the 0nm/In0.06Ga0.94N and 2nm/In0.06Ga0.94N samples, respectively. These results agree well with the values computed from Eq. 3-14. The turn-on voltages for the same samples are ~0.8, ~1.1 and ~1.0 V, respectively, as a result of the increased effective barrier height. The forward I-V calculations are based on Eq. 3-13, and the image force lowering and bias dependent effective barrier height are considered as well. The values of the parameters used for all calculations (including forward and reverse I-V curves) in this work are summarized in Table 3-2. The experimental I-V curves of the In0.1Ga0.9N-containing samples appear to consistently exhibit excess current in the low forward bias region as shown in Figure 43 3-6(b). The distinctive two-region like I-V characteristics may indicate two current mechanisms exist in the In0.1Ga0.9N-containing samples. One component is the TE current which dominates in the high forward bias region; the other may be defectrelated tunneling (TU) current which dominates in the low forward bias region. Lower growth temperature for the higher-In-concentration InGaN layers may have induced more defects. The calculated TE current for the In0.1Ga0.9N-containing samples fits the experimental curves in the high forward bias region reasonably well. More discussions on the defect-related current will be discussed in the section 3.4. Figure 3-6 Forward I-V curves of the five samples with areas of 5×10-5 cm2. (a) Control and In0.06Ga0.94N-containing samples, (b) Control and In0.1Ga0.9N-containing samples. The colored dots are measurement data, the solid lines are calculated TE currents and the dash lines are drawn TU currents. 44 Table 3-2 Values of the parameters used for all calculations (including forward and reverse I-V curves) in this work.a Nd (n- GaN) 1.0~1.1×1017 cm-3 t (InGaN) 15 nm b0 0.95~1.05 eV Nd (InGaN) 3.5~4.5×1017 cm-3 b t (GaN cap) 2 nm Ec (In0.06Ga0.94N) 0.09 eV k Nd (GaN cap) 5×1016 cm-3 c (In0.06Ga0.94N) 1.7~2.0×1012 cm-2 g Ec (In0.1Ga0.9N) 0.18~0.22eV l GaN 8.9× d (In0.1Ga0.9N) 2.6~3.0×1012 cm-2 h m* 0.2×m0 m In0.06Ga0.94N 9.28× e A* 26.4 Acm-2K-2 i Rs 30~70 In0.1Ga0.9N 9.54× f Aj 5.0×10-5 cm2 T 300 K a The other parameters used in the calculations but not listed here are all theoretical physical constants, e.g. q and k etc. b, c The UID InGaN and GaN are expected to be n-type doped. Reference . d, e, f 0 = 8.85×10-14 F/cm is the dielectric constant of vacuum. InxGa1-xN is linearly interpolated values from GaN = 8.9×0 and InN = 15.3×0. Reference . g, h Estimated values by C-V measurements discussed above. i Reference . j A is the diode area. k, l Reference . m Reference . 3.2.3 Reverse I-V measurements and analysis Diodes with different areas for all different layer stack designs (as specified in Table 3-1) were fabricated and measured to study the reverse leakage current as a function of diode diameter at fixed reverse bias. The measurement results show that the leakage current is approximately proportional to the corresponding area of the diodes (instead of the diameters), indicating that the leakage current is not dominated by edge effects. Leakage currents of two representative cases (control and 0nm/In0.06Ga0.94N) measured at reverse bias of 50 V are plotted against diode areas, as 45 shown Figure 3-7. The curves suggest that there is a slightly superlinear increase of the leakage current with the diode area. We attribute this effect to a small change in effective Schottky barrier height (SBH) with the diode area. Such a reduction of effective SBH with diode area is also consistent with the experimentally observed forward I-V curves. This effect can be attributed to the fact that the effective SBH can be reduced by the presence of defects, and with increasing diode area (and correspondingly a wider range of defects) the distribution of local effective SBHs across the sample is likely to extend to lower values. More detailed analysis of the effects of the defects on the electrical characteristics of InGaN/GaN Schottky diodes will be discussed in the following sections. Figure 3-7 Currents at reverse bias 50 V as a function of diode area for the control and 0nm/In0.06Ga0.94N samples. The colored dots are measurement data with 10% error bars and the solid lines are linearly fitting curves. The experimental and calculated reverse I-V curves are shown in Figure 3-8. For the experimental results shown in Figure 3-8(a), the InGaN surface layer designs significantly reduce the leakage current under high reverse bias. Furthermore, it is 46 seen that the suppression of leakage current is more effective for layer designs without GaN cap (0nm/In0.06Ga0.94N and 0nm/In0.1Ga0.9N) as predicted in Figure 3-3(c). However, it is also noted that the leakage current reduction of the In0.1Ga0.9Ncontaining samples is less than expected. This corresponds well with the less than expected polarization charge density at the In0.1Ga0.9N/GaN interface, as extracted from the C-V results. The calculated curves based on Eq. 3-1, fit the experimental curves well in high reverse bias regime as shown in Figures 3-8(b) and 3-8(c). In the cases of control, 2nm/In0.06Ga0.94N and 0nm/In0.06Ga0.94N samples, the last several experimental data points are higher than the calculated values, which is probably due to impact ionization effects at very high surface electric field conditions as mentioned before. In the lower reverse bias regime, the leakage current is expected to be dominated by mechanisms other than direct tunneling described by Eq. 3-1, such as trap/defect center-assisted tunneling and/or generation current. 47 Figure 3-8 Reverse I-V curves of the five samples with area of 5×10-5 cm2. (a) Experimental curves, (b) Experimental and calculated curves of the control and In0.06Ga0.94N-containing samples, (c) Experimental and calculated curves of the control and In0.1Ga0.9N-containing samples. The colored dots are measurement data and the solid lines are calculated curves. Significant improvement is also observed in the breakdown voltages for the InGaN surface layer designs which exhibit an increase of ~40 V with respect to the control sample. A histogram of the breakdown voltages for the control and InGaN- 48 containing samples is shown in Figure 3-9. To ensure the validity of this statistics, the data of the control and InGaN-containing diodes shown here come from different fabricated samples and different grown wafers. Figure 3-9 The histogram of the breakdown voltages for the control and InGaNcontaining diodes. 3.3 Leakage current reduction using higher pressure GaN buffer MOCVD grown III-N epitaxial layers suffer from high dislocation density due to the highly lattice-mismatched growth substrates, such as the sapphire used in this work . The excess reverse leakage current of the III-N-based Schottky diodes has been reported to be dislocation related , . It has also been reported that compared to conventional low-pressure (LP) MOCVD growth, the higher pressure (HP) MOCVD growth technique favors reduction of the dislocation density, and 49 growth of high-quality GaN layers, although there will be an increase in the gas-phase parasitic reactions , . In our work, we applied the HP MOCVD growth technique to the GaN buffer layer to reduce the dislocation density but used the LP MOCVD growth for other layers to minimize the parasitic gas-phase reactions. For comparison purposes, a control and a 2nm/In0.1Ga0.9N samples using HP GaN buffer were grown, labeled as Control_HP and 2nm/In0.1Ga0.9N_HP, respectively. The growth and fabrication details are the same as for the samples discussed above, except the higher growth pressure of the GaN buffer layer as shown in Table 3-1. The full width at half maximum (FWHM) of the (0002) XRD rocking curve of the samples using HP GaN buffer was ~284 arcsec, in comparison with the ~337 arcsec of the samples using LP GaN buffer, indicating lower dislocation density and the better layer quality . As shown in Figure 3-10, the corresponding reverse I-V curves of the samples using HP GaN buffer exhibit significantly less leakage current and higher breakdown voltages compared to that of the samples using LP GaN buffer. 50 Figure 3-10 Reverse I-V curves of the samples using HP and LP GaN buffer layers with area of 5×10-5 cm2. (a) Experimental curves, (b) Experimental and calculated curves of the Control and Control_HP samples, (c) Experimental and calculated curves of the 2nm/In0.1Ga0.9N and 2nm/In0.1Ga0.9N_HP samples. The colored dots are experimental data and the solid lines are calculated curves. We verified by C-V measurements that the improved characteristics are not the result of changed doping level, since we measured Nd ≈ 1×1017 cm-3 for the n- GaN 51 layer for the samples with both types of GaN buffers. As shown in Figure 3-10(b) and (c) and 3-11, the significantly reduced leakage current and the forward current for the samples using HP GaN buffer can be fit with the expressions outlined above, with only increasing SBHs by 0.1 and 0.05 eV for the Control_HP and 2nm/In0.1Ga0.9N_HP samples compared to the Control and 2nm//In0.1Ga0.9N samples, respectively. In Figure 3-11, the defect-related current is not observed in the low forward bias region for the samples using HP GaN buffer, which indicates lower defect densities in these samples. This is consistent with our XRD measurement results. In Figure 3-12, the histogram of the extracted SBHs from the experimental forward I-V curves also exhibits an average of ~0.1-eV higher SBH for the Control_HP samples relative to the Control samples. The significant SBH increase of the samples using HP GaN buffer can be attributed to the different defects densities in the materials caused by the different buffer layer growth pressures. More detailed studies and explanations will be presented in the following section. 52 Figure 3-11 Forward I-V curves of the Control_HP and 2nm/In0.1Ga0.9N_HP samples with area of 5×10-5 cm2. The colored dots are experimental data and the solid lines are calculated TE currents. Figure 3-12 The histogram of SBHs extracted from the experimental forward I-V curves of the Control and Control_HP samples. 3.4 InGaN/GaN material growth and characterization 53 All materials were grown using a Thomas Swan close-coupled showerhead 3×2’’ MOCVD system. Material characterizations including the investigations of surface morphology, defects, electrical and thermal properties were carefully performed. 3.4.1 InGaN/GaN MOCVD growth Figure 3-13 shows the Thomas Swan close-coupled showerhead (CCS) 3×2’’ MOCVD system. This commercial MOCVD reactor uses vertical laminar flow technology in which group Ⅲ (TMGa, TEGa, TMAl and TMIn) and group Ⅴ (NH3) precursors enter separately into the reaction chamber through the showerhead. The precursors’ pre-reactions are effectively avoided. The showerhead has a high density of 100 tubes/inch2 with a tube diameter of 0.6 mm which ensures the uniformity of the gas flow into the reactor chamber. Moreover, the system provides the adjustment of the showerhead to susceptor gap in the range of 5 mm to 25 mm. With this adjustment, a better quality GaN film with lower threading dislocation density (estimated by XRD rocking curve) can be grown, which we believe is due to the reduction of the residence time of the precursors (less parasitic gas phase reaction) in the reactor chamber. 54 Figure 3-13 Thomas Swan close-coupled showerhead (CCS) 3×2’’ MOCVD system. A: Metal-organic sources cabinet; B: Glove box; C: Reactor chamber; D: Showerhead; E: Susceptor. For growing GaN on c-Sapphire using MOCVD, we used the traditional lowtemperature (LT: 530 oC) GaN nucleation layer method followed by high-temperature (HT: 1040 oC) GaN buffer layer for the material growth . The substrates used were 2-inch c-plane sapphire with a 0.1-degree off-cut towards the m-plane. Trimethylgallium (TMGa), ammonia (NH3) and silane (SiH4) were used as Ga, N precursors and n-type Si dopant, respectively; for InGaN growth, Triethylgallium (TEGa), Trimethylindium (TMIn) and NH3 were used as Ga, In and N precursors, respectively. H2 and N2 were used as carrier gases for GaN and InGaN growth, 55 respectively. Thick InGaN samples (> 300 nm to ensure full strain relaxation ) were grown for estimating the indium concentration and optimizing the InGaN growth by X-ray diffraction (XRD) measurements. Figure 3-14 shows the dependence of indium percentage and FWHM of (0002) XRC on growth temperature and molar flow ratio of TMIn/(TMIn+TMGa). Based on these results and the design considerations discussed in section 3.2, the InGaN films used in the InGaN surface layer design were grown using TMIn, TEGa and NH3 flows of 9.26 mol/min, 8.16 mol/min and 165 mmol/min, respectively, at 820 oC for the In0.06Ga0.94N layer growth; 5.95 mol/min, 5.25 mol/min and 165 mmol/min, respectively, at 808 oC for the In0.1Ga0.9N layer growth. Figure 3-14 The indium percentage and FWHMs of (0002) X-ray rocking curve (XRC) of thick InGaN films for different growth temperatures and molar flow ratios of TMIn/(TMIn+TMGa) during growth. 56 3.4.2 InGaN/GaN material characterization As we discussed above, InGaN surface layer design can offer great benefits in increasing breakdown voltage and decreasing reverse leakage current. Additionally, InGaN/GaN, as one of the prevalent III-nitride heterostructure combinations, has attracted intense interest in relation to light emitting diodes (LEDs) , , heterojunction bipolar transistors (HBTs) , , and high power electronic devices, including power varactors , . However, the effects of film quality (especially defects) on the electrical characteristics of the InGaN/GaN Schottky diodes should also be investigated. Due to the large lattice mismatch and thermal expansion mismatch to the foreign (e.g., c-Sapphire and Si) substrates, epi-grown nitride materials suffer from a variety of defects, such as threading dislocations (TDs), stacking faults, inversion domain boundaries and nanopipes , . Although not all defects are detrimental to device performance since long-lived LEDs and lasers can be fabricated on nitride materials even with 108-cm-2 dislocation density, the effects of these defects on device characteristics are still topics of considerable interest. This section reports the observation of surface micromesa defects in InGaN/GaN materials and addresses the relationship between dislocations and surface micromesas in the InGaN/GaN system and shows that micromesas are associated with excess leakage 57 currents in InGaN/GaN Schottky barrier diodes, especially at higher annealing temperatures. 188.8.131.52 Reported defects in GaN and InGaN materials Previous work has elucidated many of the characteristics of GaN and InGaN defects. Nanopipes, with radii of 35 to 500 Å, in MOCVD-grown GaN epi-layers were first reported by Qian et al . Their scanning force microscopy (SFM) and highresolution transmission electron microscopy (TEM) studies revealed that the nanopipes are open cores of screw TDs . These hollow pipes were predicted earlier by Frank, who noted that for a dislocation whose Burgers vector exceeds a critical value, there exists a local equilibrium state in which the dislocation core is an empty tube . Similar defects, named micropipes (with sizes more than two orders of magnitude larger than those of the nanopipes observed in GaN), are frequently observed in SiC, another wide bandgap semiconductor with hexagonal crystal structure , . The micropipes in SiC can be observed by optical microscope and have been reported to be detrimental to the performance of devices. Neudeck et al. reported that micropipes are the main source of electrical breakdowns in SiC p-n junction diodes and limiting factors for applications of SiC in high-power, highfrequency, and high-temperature electronic devices , . In contrast to the micropipes in SiC, the nanopipes in GaN cannot be observed by optical microscopy because of their small sizes; usually TEM or wet chemical etching techniques are 58 required to observe them, , . Therefore, it is difficult to study the direct correlation between the nanopipes and the electrical characteristics of the nitride devices. In this section, we investigated the surface defects in MOCVD-grown InGaN/GaN materials by Nomarski optical microscopy (NOM), scanning electron microscopy (SEM) and atomic force microscopy (AFM). Different growth pressures for GaN buffer layers were used to vary the material defect density , . After adding a thin surface layer of InGaN, micro-scale surface mesas were observed by NOM. We were able to use a large-scale defect mapping method before and after hot phosphoric acid (H3PO4) etching to analyze the origin of the surface micromesas and relate them to nanopipes. Direct NOM observation of the micromesas allowed us to study the effects of micromesas, and by inference, nanopipes, on reverse leakage current in Ni-InGaN/GaN Schottky barriers. Detailed surface topography of micromesas was investigated by SEM and AFM. We previously discussed the breakdown characteristics improvement of GaN Schottky diodes by adding a thin InGaN surface layer. Here we further study the reverse leakage current in InGaN/GaN Schottky barriers with extensive measurements of reverse leakage current versus diode dimension and micromesa number before and after thermal annealing at different temperatures. We show an increase of leakage current with thermal annealing, which is sometimes an essential step in device fabrication (e.g. thermally curing polymers for metal isolation). RBS measurements are also used to study the inter-diffusion between Ni and InGaN/GaN at different annealing temperatures. We conclude that the micromesas are the main source of leakage in these structures. We show that high 59 pressure epitaxial growth can significantly reduce micromesa density and thus leakage current. 184.108.40.206 Experimental procedures The structure of the Schottky barrier diodes investigated in this section is shown in Figure 3-15(a). The materials were processed into circular mesa diodes of the form illustrated in Figure 3-15(b). The Nomarski micrograph of the diode illustrated shows the presence of surface micromesas. Figure 3-15 a) Schematic cross section of the InGaN/GaN Schottky diode and (b) the Nomarski optical microscopy top view of a real diode with surface micromesas. Growth details and sample labels are summarized in Table 3-3. Low pressure (LP) growths utilized 300 mbar pressure for the buffer layer growth, while high pressure (HP) samples employed 900 mbar in this step. The HP (near-atmosphere pressure) buffer layer growth was found to reduce the defect density , . For HP_InGaN/GaN and LP_InGaN/GaN samples, there were ~ 10-nm InGaN surface 60 layers grown on top. After the MOCVD growth, the wafers were diced into 1 × 1 cm2 squares for various experiments. Table 3-3 Sample labels and key growth details used in this work.a Sample LP_GaN LP_InGaN/GaN HP_ GaN HP_InGaN/GaN labels InGaN ~6% In, ~10 nm, 400 N.A. layer mbar, 808 oC ~6% In, ~10 nm, 400 N.A. mbar, 808 oC n- GaN (n≈1×1017 cm-3, 1 m), 200 mbar, 1040 oC n+ GaN (n≈5×1018 cm-3, 1.5 m), 200 mbar, 1040 oC Common GaN buffer (~1.5 m), 300 mbar for low pressure (LP), 900 mbar for layers high pressure (HP) GaN buffer, 1040 oC Low-temperature GaN nucleation layer (~20 nm), 600 mbar, 530 oC c-Sapphire substrate a The coalescence time for HP buffer and LP buffer is ~50 mins and ~10 mins, respectively; the growth rate for HP buffer an LP buffer is ~0.52 nm/s and ~0.46 nm/s, respectively; and the InGaN growth rate is ~0.0326 nm/s. 220.127.116.11 X-ray diffraction measurements Full width at half maximum (FWHM) of symmetric (0002) and asymmetric (10-12) x-ray rocking curves (XRCs) were measured to compare the threading dislocation densities in these four samples. The results are included in Table 3-4. It is known that the FWHM of the symmetric (0002) XRC is broadened by screw- and 61 mixed-type threading dislocations and the asymmetric (10-12) XRC is broadened by all TDs , . Narrower FWHM of the samples (HP_GaN and HP_InGaN/GaN) using higher growth pressure for GaN buffer layers indicates lower edge-, screw- and mixed-type TD densities than those of the samples (LP_GaN and LP_InGaN/GaN) using low pressure growth for GaN buffer layers. Table 3-4 FWHM of symmetric (0002) and asymmetric (10-12) XRCs, surface micromesa density estimated under Nomarski optical microscopy and nanopipe and TD densities estimated by EPD in all samples. FWHM of Micromesa density Nanopipe TD density (0002)/(10-12) by NOM (before density by EPD by EPD from XRCs (arcsec) etch) (cm-2) (cm-2) AFM (cm-2) HP_InGaN/GaN 276/325 1.6×105 1.9×105 1.5×108 LP_InGaN/GaN 347/476 5.8×105 6.8×105 2.8×108 HP_GaN 281/334 0 2.5×105 1.6×108 LP_GaN 338/440 0 9.1×105 3.0×108 Sample label 18.104.22.168 Nomarski microscope imaging Smooth surfaces are observed for the GaN-only (LP_GaN and HP_GaN) samples, while large surface mesas, with density in the range of 105 cm-2, are optically observable on the LP_InGaN/GaN and HP_InGaN/GaN samples as shown in Figure 3-16 with only ~ 10-nm InGaN top layers. These surface mesas are typically 1~2 m in diameter and less than 30 nm in height on our ~10-nm InGaN containing samples from NOM and AFM measurements. Corresponding with lower TD density estimated 62 by XRC measurements, the InGaN/GaN sample grown using higher growth pressure for the GaN buffer layer also shows a much lower surface micromesa density as shown in Table 3-4. Figure 3-16 Nomarski optical microscopy images of (a) HP_InGaN/GaN, (b) LP_InGaN/GaN, (c) HP_GaN and (d) LP_GaN. The inset in (b) is a zoom-in image of one surface micromesa. 22.214.171.124 Surface topography investigation by SEM and AFM Representative SEM and AFM micrographs of the surface micromesas on InGaN/GaN samples are shown in Figure 3-17. The micromesa shows spiral steps, which typically emerge from a nanopipe. By carefully examining the height of the 63 different resolvable steps showing in Figure 3-17(b), the step heights were found to be around several nanometers, roughly with a greatest common divisor (GCD) of 5.4±0.3 Å. This GCD is consistent with the expected value of c-lattice constant of InGaN (5.19 Å and 5.69 Å for GaN and InN, respectively) . The measured step heights that are integer multiples (typically 2~4) of the GCD (~ c-lattice constant of InGaN) are consistent with the step sizes reported for growth spirals in other material systems, and can be attributed to step bunching . Figure 3-17 Representative SEM and AFM (tapping mode) micrographs of the surface micromesas. (a) A SEM micrograph; (b) An AFM micrograph; (c) 3-D AFM micrograph of (b); and (d) surface profile along the line shown in (b). (b), (c) and (d) are from the same micromesa and (a) is from a different one. Numbers in (b) indicate the resolvable spiral steps. 64 126.96.36.199 Etch pit density measurements All samples were immersed into 180-oC H3PO4 for 7 minutes to perform the etch pit density (EPD) measurements , and followed by NOM, SEM and AFM investigations to analyze the etch pit type and density. Figure 3-18 shows the AFM images of the etched HP_InGaN/GaN and LP_InGaN/GaN samples and their corresponding surface profiles. The TD densities in the range of 108 cm-2 in these samples can be estimated by counting the etch pits in these images. Figure 3-18 10 × 10 m2 AFM images of (a) HP_InGaN/GaN, (b) surface profile along the line in (a), (c) LP_InGaN/GaN, and (d) surface profile along the line in (c) after H3PO4 etch. 65 Although the SEM and AFM micrographs in Figure 3-17 show that the surface micromesas grow spirally around the nanopipes, the scanning areas for these two techniques are too small to conclusively identify the origin of the surface micromesas. Therefore, for the LP_InGaN/GaN sample, surface micromesas (before etch) and etch pits were mapped using NOM over a large area for further characterization. For better comparison, two representative small parts of the zoomed-in mapped images are shown in Figure 3-19. The small etch pits that correspond to the TDs shown in the AFM images cannot be observed by NOM. The observable etch pits (black dots) under the NOM shown in Figure 3-19(b) represent the same type of defect as the large etch pit shown in the AFM image in Figure 3-18(c) (indicated by an arrow), which is clearly different from the other small TD-related etch pits in the AFM images. These large etch pits have a density in the range of 105 cm-2, which is three orders of magnitude lower than the TD density. 66 Figure 3-19 Surface micromesa mapping by Nomarski optical microscopy. (a) Surface micromesas before etch and (b) etch pits in the same area of a LP_InGaN/GaN sample. (c) A schematic superposition of image (a) and (b). The inset in (b) is a representative SEM image of a large etch pit shown in (b). The circles and dots in (c) represent the surface micromesas and nanopipe-related etch pits, respectively. 67 188.8.131.52 Discussion of material defect characterization Hong et al. performed thorough TEM studies of the origin of the hexagonalshaped etch pits in (0001) GaN films, and concluded that these etch pits with a density 2~4 orders of magnitude lower than the TD density originated from nanopipes (opencore screw TDs) , . The 105 cm-2 EPD that was measured is also quite close to those reported nanopipe densities in MOCVD-grown GaN films , . Based on our consistent observations with their TEM studies, we believe that the large etch pits in the AFM and NOM images originate from nanopipes. Furthermore, from the mapping images shown in Figure 3-19, it can be clearly seen that most of the surface micromesas (~ 80%) form nanopipe-related etch pits. This is consistent with the micromesa observations under SEM and AFM shown in Figure 3-17. In accordance with the aforementioned TEM studies, the hexagonalshaped etch pit shown in the inset of Figure 3-19(b) is formed by etching along the nanopipe at the center of the micromesa shown in Figure 3-17. Indium incorporation at lower growth temperatures is considered an important factor in the formation of surface micromesas, since no surface micromesas were observed on the GaN-only samples. Indium atoms have much higher surface mobility on the GaN surface than Ga atoms at the lower InGaN growth temperature, giving them higher probability to occupy the lowest energy sites and form spiral steps around the nanopipes , . The roughly extracted c-lattice constant value of 5.4±0.3 Å from the AFM micrograph 68 of the surface micromesa also suggests a high indium concentration in the micromesa area. The indium segregation around nanopipes (open-core screw TDs) has also been observed by energy dispersive x-ray (EDX) measurements in InAlN/GaN systems . Therefore, we may speculate that the surface micromesa is formed by indiumrich spiral growth around nanopipes at lower InGaN growth temperatures with a growth rate that is higher than that of the planar growth on the remaining GaN surface. As shown schematically in Figure 3-19(c) with the superposition of the two mapping images, some surface micromesas that do not form nanopipe-related etch pits and some nanopipe-related etch pits that do not correspond to optically observable micromesas were also observed. Figure 3-20 shows corresponding micrographs of the surface micromesas (with and without nanopipes at the center) and a nanopipe (without formation of a surface micromesa) that were found consistent with the observations in the mapping images in Figure 3-19(c). The former case could be attributable to the formation of surface micromesas around some defect other than a nanopipe (e.g. stacking fault within the InGaN layer due to strain relaxation) ; the latter case could be due to inhibition of spiral growth around nanopipes due to the local strain in the InGaN layer. These tentative explanations, however, need to be further investigated. Table 3-4 summarizes the results of XRC measurements and surface micromesa and TD densities for the four samples. The surface micromesa, nanopipe, and TD densities in HP_GaN and HP_InGaN/GaN samples are lower as expected, which is consistent with their narrower FWHM of XRCs. In the InGaN/GaN samples, the surface micromesa density of ~105 cm-2 is close to the nanopipe density and much 69 lower than the TD density of ~108 cm-2. This is also a good indication that the surface micromesas have a close relationship with nanopipes but little relationship with other TDs. In addition, the reduction of nanopipe-related EPD by adding a thin InGaN surface layer (9.1×105 cm-2 to 6.8×105 cm-2 between LP_GaN and LP_InGaN/GaN, and 2.5×105 cm-2 to 1.9×105 cm-2 between HP_GaN and HP_InGaN/GaN, respectively) is significant. However, the additional InGaN surface layer does not introduce too much TD density change. This observation is in agreement with Ono et al.’s work . Figure 3-20 An AFM (tapping mode) micrograph of surface micromesas with and without nanopipes at the center. The inset is a SEM image of a nanopipe without formation of a surface micromesa on the InGaN/GaN sample. 70 3.4.3 Electrical characteristics of InGaN/GaN Schottky diodes HP_InGaN/GaN and LP_InGaN/GaN samples were fabricated into Schottky diodes with different diameters in the range of 17 m to 280 m, followed the fabrication procedure mentioned in section 2-1, to investigate their electrical characteristics. The I-V characteristics were measured on different sizes of diodes. The relation between leakage current at a reverse bias (Vr) of 30 V and diode diameter is shown in Figure 3-21. The data trend which follows the slope-of-two line (except for the smallest HP_InGaN/GaN diodes) on a logarithmic scale indicates that the leakage current is proportional to the corresponding area of the diodes, instead of being dominated by edge effects. The HP_InGaN/GaN Schottky diodes with lower surface micromesa and nanopipe density showed about two orders of magnitude lower leakage current than that of LP_InGaN/GaN diodes. From the estimated micromesa density shown in Table 3-4, the average area per micromesa is 625 m2 for HP_InGaN/GaN and 172 m2 for LP_InGaN/GaN, which in turn correspond to critical diameters Dc of 28 m and 15 m, respectively. Diodes without micromesas are expected to occur (on a probabilistic basis) when diode diameter becomes close to or smaller than Dc. As seen from Figure 3-21, the smallest LP_InGaN/GaN Schottky diodes with diameters of 17 m (close to the value of Dc for this wafer of 15 m), showed large scattering of leakage currents around their slope-of-two trend; the smallest HP_InGaN/GaN Schottky diodes with diameters of 17 m (much smaller than the value Dc of for this 71 wafer, 28m) showed significantly lower leakage current than their slope-of-two trend. This suggests that the micromesas are likely a major leakage path in the InGaN/GaN Schottky diodes. Figure 3-21 Leakage current at a reverse bias of 30 V versus diode diameter for LP_InGaN/GaN and HP_InGaN/GaN Schottky diodes. The black dashed lines have slope of two and the color dashed curves represent the trend of measured data points. To confirm the relationship, the number of micromesas for each of the smallest (17-m diameter) Ni-InGaN/GaN Schottky diodes was first counted under NOM and then a study of their forward and reverse I-V characteristics was performed. Figure 322 shows the relation between leakage current at Vr = 30 V and micromesa number on the smallest diodes. It is clear that the leakage current increases with the increase of micromesa number. Representative forward I-V curves for the smallest diodes without and with surface micromesas are shown in Figure 3-23. In Figure 3-23(a), the I-V curve for the diode without surface micromesa has an ideality factor of ~1.3, which is larger than unity due to the polarization charge (at the InGaN/GaN interface)-induced 72 Schottky barrier height (SBH) increase as forward bias increases as we discussed in section 3.2.2. The corresponding calculations based on thermionic emission (TE) theory fit the experimental curve well using Eq. 3-13. In Figure 3-23(b), I-V curves with two distinctive turn-on mechanisms were usually observed for the diodes with surface micromesas. The first turn-on mechanism in the low bias region can be modeled as due to the surface micromesa with lower SBH and higher series resistance (Rs) (due to its small area); the second turn-on mechanism, associated with the high bias region, originates from the normal InGaN/GaN Schottky barrier, with higher SBH and lower Rs. A simplistic equivalent circuit diagram for explaining this two turn-on phenomenon was also proposed in the Figure 3-23(b). In the TE-based calculations, using effective SBHs of micromesas 0.3~0.5 eV lower than effective SBHs of NiInGaN/GaN (~1.1 eV), and Rs of micromesa around two orders of magnitude larger (due to <1% micromesa area) than Rs of Ni-InGaN/GaN can match the experimental curves quite well. The lower effective SBH is likely caused by the lower conduction band edge (Ec) of InGaN and partial strain relaxation at the InGaN/GaN interface due to higher indium concentration and larger InGaN layer thickness (estimated by AFM) in the micromesa area. 73 Figure 3-22 Leakage current at a reverse bias of 30 V versus micromesa number on the smallest (17-m diameter) LP_InGaN/GaN and HP_InGaN/GaN Schottky diodes. Figure 3-23 Representative forward I-V curves for the smallest (17-m diameter) Ni-InGaN/GaN Schottky barriers (a) without surface micromesas and (b) with surface micromesas. The red dots are measured data and the solid black curves are calculated thermionic emission (TE) currents. In (b), the green and pink dashed curves represent the calculated TE currents for micromesas and InGaN/GaN, respectively. The black solid curve is the summation of the two dashed curves. The inset is the equivalent circuit diagram of the InGaN/GaN Schottky diodes with surface micromesas. 74 Representative reverse-bias I-V curves and the corresponding calculated curves for the smallest InGaN/GaN Schottky diodes are shown in Figure 3-24. The calculations based on electron tunneling through the Schottky barrier under reverse biases fit the experimental curves well in the high-bias regime as we discussed in section 3.1. In the low-bias regime, the tunneling current is much lower than the equipment noise current and is difficult to measure. In Figure 3-24(b), it is clearly seen that when miocromesas exist, the micromesas with effective SBHs 0.3~0.5 eV lower than that of InGaN/GaN were the main source of the leakage current even though they only occupy ~ <1% area of the diode. 75 Figure 3-24 Representative reverse-bias IV curves for the smallest (17-m diameter) Ni-InGaN/GaN Schottky barriers (a) without surface micromesas and (b) with surface micromesas. The red dots are measurement data and the solid curves are calculated tunneling currents. In (b), the green curve is calculated tunneling current for micromesas and the pink curve is calculated tunneling current for InGaN/GaN. 3.4.4 Effects of thermal annealing on Ni-InGaN/GaN Schottky diodes The InGaN/GaN Schottky-diode samples were annealed in forming gas (5% H2 in N2) at different temperatures to study the effects of thermal annealing on reverse leakage current. In parallel, InGaN/GaN samples covered with ~ 100-nm Ni films were also annealed in order to study the Ni diffusion at the Ni/InGaN interface using RBS measurements. RBS measurements were carried out using 1.5 MeV 4He+ ions with a scattering angle of 150°. As shown in the measured RBS spectra in Figure 3-25, 76 for annealing at 200 oC for 60 minutes no diffusion was detected from RBS measurements; for annealing at 500 oC for 24 minutes, weak Ga and In out-diffusion were observed; for annealing at 625 oC for 15 minutes, extensive Ga and In outdiffusion and Ni in-diffusion were observed. Figure 3-25 RBS spectra of as-deposited, annealed at 200 oC for 60 minutes, 500 oC for 24 minutes and 625 oC for 15 minutes Ni-InGaN/GaN samples. The inset on the left shows the zoom-in spectra and the inset on the right is a schematic diagram of the inter-diffusion at the Ni-InGaN interface. The relation between leakage current at Vr = 30 V and the diode diameter before and after annealing at 200 oC for 1 hour and 500 oC for 24 minutes is shown in Figure 3-26. After 1-hour annealing at 200 oC, leakage current increase was significant for large-size diodes. However, the small-size diodes did not show significant leakage current increase. More data points were measured for the smallest diodes. It is seen that for the smallest HP_InGaN/GaN diodes with diameters of 17 m much smaller 77 than their Dc of 28 m showed little leakage current degradation after 200-oC annealing. Although the RBS measurement did not detect any diffusion at 200-oC annealing, the results of leakage current versus diameter (reverse leakage degradation only observed for larger diodes that contain surface micromesas) suggest that the surface micromesas with nanopipes at their center were likely an easy diffusion path at lower temperatures (e.g. 200 oC). This diffusion, however, is difficult to measure by RBS due to <1% diode area for the surface micromesas. Diffusion through surface micromesas would degrade the Schottky barriers, so the smallest diodes without surface micromesas would not be affected by the 200-oC annealing. This was confirmed by experimental data. Similar metal diffusion through the cores of TDs in GaN-based LEDs was already observed at higher temperatures (> 600 oC) under TEM by Hsu et al . The reverse-bias IV curves can be also fitted using tunneling current calculations (not shown) by lowering the SBH of micromesas by ~0.07 eV from the SBH value used before annealing. After 24-minute annealing at 500 oC, all diodes showed significant leakage current increase and some LP_InGaN/GaN diodes suffered breakdown at Vr < 30 V. This suggests that extensive diffusion started at the Ni/InGaN interface and degraded the Ni-InGaN/GaN Schottky barriers (leading to ~0.25 eV SBH lowering relative to the SBH value used before annealing according to the tunneling current calculations). This is also consistent with our RBS measurements. 78 Figure 3-26 Leakage current at a reverse bias of 30 V versus diode diameter for LP_InGaN/GaN and HP_InGaN/GaN Schottky diodes before and after annealing at different temperatures. 3.5 Application for enhancement-mode HFETs As we discussed above, the InGaN surface layer design can increase the effective Schottky barrier height, increase the electron tunneling distance under reverse biases and improve reverse breakdown and leakage characteristics. Also the design can be used to achieve enhancement-mode GaN-based HEMTs (conventional AlGaN/GaN HEMT is a depletion-mode device), which are more favorable in many circuit applications for reducing the circuit design complexity (e.g., eliminating the need for negative-polarity voltage supply) and fail-safe operations. In fact, the enhancement-mode GaN-based HEMTs have been reported using the InGaN surface 79 layer design on AlGaN/GaN HEMTs , . Other than the InGaN surface layer design, an InGaN layer underlying the conventional AlGaN/GaN HEMT structure designed as an electron back barrier was also reported . In this section, we also simulated the InGaN surface layer design in the AlGaN/GaN HEMT structure to illustrate the mechanism for enhancement-mode operations. The simulated (with a Silvaco ATLAS 2-D simulator) structures for the conventional AlGaN/GaN HEMT and the AlGaN/GaN HEMT with InGaN surface layer design, as well as the corresponding energy band diagrams are shown in Figure 3-27. The polarization charges at the AlGaN/GaN and InGaN/AlGaN interfaces were assumed to be 1×1013 cm-2 and -2.1×1013 cm-2, respectively , . It is clearly seen that with the InGaN surface layer design, the effective Schottky barrier height of ~ 3.4 eV is much higher than that (~1.8 eV) of the conventional design. Therefore, the InGaN/AlGaN/GaN HEMT is more pinched off under the gate at zero bias with a 2-D electron-gas (2DEG) density of 1×1011 cm-2, in comparison with the 2DEG density of 3×1012 cm-2 for the conventional AlGaN/GaN HEMT. 80 Figure 3-27 Simulated AlGaN/GaN and InGaN/AlGaN/GaN HEMT structures and the corresponding energy band diagrams. (a) Conventional AlGaN/GaN HEMT structure, (b) InGaN/AlGaN/GaN HEMT structure for enhancement-mode operation, (c) conduction band diagram under the Ni gate at zero bias for the structure (a) and (d) conduction band diagram under the Ni gate at zero bias for the structure (b). I-V characteristics of these two devices were also simulated. Figure 3-28 showed the corresponding drain current (Id) vs drain voltage (Vd) and drain current versus gate voltage (Vg) for both of AlGaN/GaN and InGaN/AlGaN/GaN HEMTs. It is observed from these curves that the threshold voltage (Vt) is increased by ~ 2 V (from ~-2 V to ~0 V) by using the InGaN surface layer. It can be expected that the enhancement-mode operation with even higher Vt (>0 V) can be obtained with more 81 optimized epitaxial layer structure and/or different gate schemes (e.g., a MISHFET structure). 82 Figure 3-28 Simulated I-V characteristics for AlGaN/GaN and InGaN/AlGaN/GaN HEMTs. (a) Id versus Vd for AlGaN/GaN HEMT, (b) Id versus Vd for InGaN/AlGaN/GaN HEMT and (c) Id versus Vg for both HEMTs. 83 3.6 Summary of InGaN/GaN technology Leakage-current reduction and breakdown voltage increase in GaN Schottky barriers were achieved by the incorporation of suitable InGaN surface layers. Analysis shows that the InGaN surface layers change the electric-field distribution near the surface due to polarization-induced charges. Experimental C–V and I–V measurements confirm this analysis. The HP-MOCVD-growth technique of the GaN buffer layer was also found to be effective in reducing the leakage current and increasing the breakdown voltage of GaN Schottky barriers. Additionally, surface micromesas were observed on InGaN/GaN epi-layers, and their characteristics and origin were investigated by NOM, SEM and AFM. Large-scale mapping between surface micromesas and etch pits under NOM revealed that most of the surface micromesas originated from nanopipes in GaN. Studies of RBS and the electrical characteristics on corresponding Ni-InGaN/GaN Schottky barriers indicated that the surface micromesas with nanopipes at the center were the main source of reverse leakage current and caused an easy metal diffusion path, even in relatively low-temperature thermal annealings. This diffusion through nanopipes is detrimental to the electrical characteristics of Ni-InGaN/GaN Schottky barriers. The use of an HP GaN buffer layer effectively reduced the nanopipe and surface micromesa densities. However, in 84 order to further improve the electrical characteristics of the InGaN/GaN material, methods for further reducing or terminating surface micromesas on the surface (e.g. with thin surface dielectrics) are needed. Finally, the application of InGaN surface layer design in AlGaN/GaN HEMTs for achieving enhancement-mode operation is introduced. Section 3.1, 3.2 and 3.3, are a rearrangement of the paper “Analysis of Reverse Leakage Current and Breakdown Voltage in GaN and InGaN/GaN Schottky Barriers,” Wei Lu, Lingquan Wang, Siyuan Gu, David P. R. Aplin, Daniel M. Estrada, Paul K. L. Yu, and Peter M. Asbeck, IEEE Trans. Electron Devices, vol. 58, no. 7, pp. 1986– 1994, Jul. 2011. The dissertation author was the primary author of the paper. Section 3.4, is a rearrangement of the paper “Effects of surface micromesas on reverse leakage current in InGaN/GaN Schottky barriers,” Wei Lu, Tomoaki Nishimura, Lingquan Wang, Tohru Nakamura, Paul K. L. Yu, and Peter M. Asbeck, J. Appl. Phys., vol. 112, pp.044505, Aug. 2012. The dissertation author was the primary author of the paper. 85 3.7 Reference  Q. Chen, J.W. Yang, A. Osinsky, S. Gangopadhyay, B. Lim, M. Z. Anwar, M. A. Khan, D. Kuksenkov, and H. Temkin, “Schottky barrier detectors on GaN for visible-blind ultraviolet detection,” Appl. Phys. Lett., vol. 70, no. 17, pp. 2277–2279, Apr. 1997.  M. Ali, V. Cimalla, V. Lebedev, H. Romanus, V. Tilak, D. Merfeld, P. Sandvik, and O. Ambacher, “Pt/GaN Schottky diodes for hydrogen gas sensors,” Sens. Actuators B, Chem., vol. 113, no. 2, pp. 797–804, Feb. 2006.  Z. Z. Bandic, P. M. Bridger, E. C. Piquette, T. C. McGill, R. P. Vaudo, V. M. Phanse, and J. M. Redwing, “High voltage (450 V) GaN Schottky rectifiers,” Appl. Phys. Lett., vol. 74, no. 9, pp. 1266–1268, Mar. 1999.  W. Lu, L. Wang, S. Gu, D. P. R. Aplin, D. M. Estrada, P. K. L. Yu, and P. M. Asbeck, “InGaN/GaN Schottky diodes with enhanced voltage handling capability for varactor applications,” IEEE Electron Device Lett., vol. 31, no. 10, pp. 1119–1121, Oct. 2010.  E. J. Miller, D. M. Schaadt, E. T. Yu, P. Waltereit, C. Poblenz, and J. S. Speck, “Reverse-bias leakage current reduction in GaN Schottky diodes by electrochemical surface treatment,” Appl. Phys. Lett., vol. 82, no. 8, pp. 1293– 1295, Feb. 2003.  V. Adivarahan, G. Simin, J. W. Yang, A. Lunev, M. A. Khan, N. Pala, M. Shur, and R. Gaska, “ SiO2-passivated lateral-geometry GaN transparent Schottky-barrier detectors,” Appl. Phys. Lett., vol. 77, no. 6, pp. 863– 865, Aug. 2000.  M. L. Lee, J. K. Sheu, W. C. Lai, S. J. Chang, Y. K. Su, M. G. Chen, C. J. Kao, G. C. Chi, and J.M. Tsai, “GaN Schottky barrier photodetectors with a low-temperature GaN cap layer,” Appl. Phys. Lett., vol. 82, no. 17, pp. 2913– 2915, Apr. 2003.  H. Jiang, T. Egawa, H. Ishikawa, Y. B. Dou, C. L. Shao, and T. Jimbo, “ Barrier-height-enhanced n-GaN Schottky photodiodes using a thin p-GaN surface layer,” Jpn. J. Appl. Phys., vol. 43, no. 7A, pp. 4101–4104, Jul. 2004. 86  K. Matsumoto and A. Tachibana, “Growth mechanism of atmospheric pressure MOVPE of GaN and its alloys: Gas phase chemistry and its impact on reactor design,” J. Cryst. Growth, vol. 272, no. 1–4, pp. 360– 369, Dec. 2004.  F. A. Padovani and R. Stratton, “Field and thermionic-field emission in Schottky barriers,” Solid State Electron., vol. 9, no. 7, pp. 695–707, Jul. 1966.  T. Hashizume, J. Kotani, and H. Hasegawa, “Leakage mechanism in GaN and AlGaN Schottky interfaces,” Appl. Phys. Lett., vol. 84, no. 24, pp. 4884–4886, Jun. 2004.  C. Y. Chang and S. M. Sze, “Carrier transport across metalsemiconductor barriers,” Solid State Electron., vol. 13, no. 6, pp. 727–740, Jun. 1970.  C. R. Crowell and V. L. Rideout, “Normalized thermionic-field (T-F) emission in metal-semiconductor (Schottky) barriers,” Solid State Electron., vol. 12, no. 2, pp. 89–105, Feb. 1969.  P. Hacke, T. Detchprohm, K. Hiramatsu, and N. Sawaki, “Schottky barrier on n-type GaN grown by hydride vapor phase epitaxy,” Appl. Phys. Lett., vol. 63, no. 19, pp. 2676–2678, Nov. 1993.  M. E. Levinshtein, S. L. Rumyantsev, and M. S. Shur, Properties of Advanced Semiconductor Materials: GaN, AIN, InN, BN, SiC, SiGe. New York: Wiley, 2001.  S. Nakamura, “GaN growth using GaN buffer layer,” Jpn. J. Appl. Phys., vol. 30, no. 10A, pp. L1 705–L1 707, Oct. 1991.  H. Zhang, E. J. Miller, E. T. Yu, C. Poblenz, and J. S. Speck, “Measurement of polarization charge and conduction-band offset at InxGa1−xN/GaN heterojunction interfaces,” Appl. Phys. Lett., vol. 84, no. 23, pp. 4644–4646, Jun. 2004.  O. Ambacher, J. Majewski, C. Miskys, A. Link, M. Hermann, M. Eickhoff, M. Stutzmann, F. Bernardini, V. Fiorentini, V. Tilak, B. Schaff, and L. F. Eastman, “Pyroelectric properties of Al(In)GaN/GaN hetero- and quantum well structures,” J. Phys.: Condens. Matter, vol. 14, no. 13, pp. 3399–3434, Apr. 2002.  J. K. Sheu and G. C. Chi, “The doping process and dopant characteristics of GaN,” J. Phys.: Condens. Matter, vol. 14, no. 22, pp. R657–R702, Jun. 2002.  B. Heying, X. H. Wu, S. Keller, Y. Li, D. Kapolnek, B. P. Keller, S. P. DenBaars, and J. S. Speck, “Role of threading dislocation structure on the X- 87 ray diffraction peak widths in epitaxial GaN films,” Appl. Phys. Lett., vol. 68, no. 5, pp. 643¨C645, Jan. 1996.  J. W. P. Hsu, M. J. Manfra, R. J. Molnar, B. Heying, and J. S. Speck, “Direct imaging of reverse-bias leakage through pure screw dislocations in GaN films grown by molecular beam epitaxy on GaN templates,” Appl. Phys. Lett., vol. 81, no. 1, pp. 79–81, Jul. 2002.  P. Fini, X. Wu, E. J. Tarsa, Y. Golan, V. Srikant, S. Keller, S. P. Denbaars, and J. S. Speck, “The effect of growth environment on the morphological and extended defect evolution in GaN grown by metalorganic chemical vapor deposition,” Jpn. J. Appl. Phys., vol. 37, no. 8, pp. 4460–4466, Aug. 1998.  S. N. Lee, J. K. Son, H. S. Paek, T. Sakong, W. Lee, K. H. Kim, S. S. Kim, Y. J. Lee, D. Y. Noh, E. Yoon, O. H. Nam, and Y. Park, “Growth pressure dependence of residual strain and threading dislocations in the GaN layer,” Phys. Stat. Sol. (C), vol. 1, no. 10, pp. 2458–2461, Jul. 2004.  M. Leyer, J. Stellmach, C. Meissner, M. Pristovsek, and M. Kneissl, “The critical thickness of InGaN on (0001)GaN,” J. Cryst. Growth, vol. 310, no. 23, pp. 4913–4915, Nov. 2008.  S. Nakamura, M. Senoh, and T. Mukai, “High-Power InGaN/GaN doubleheterostructure violet light-emitting-diodes,” Appl. Phys. Lett., vol. 62, pp. 2390-2392, May. 1993.  T. Mukai, K. Kumakura, and N. Kobayashi, “Characteristics of InGaN-based UV/blue/green/amber/red light-emitting diodes,” Jpn. J. Appl. Phys Short Notes & Review Papers, vol. 38, pp. 3976-3981, Jul. 1999.  T. Makimoto, K. Kumakura, and N. Kobayashi, “High current gain (> 2000) of GaN/InGaN double heterojunction bipolar transistors using base regrowth of pInGaN,” Appl. Phys. Lett., vol. 83, pp. 1035-1037, Aug. 2003.  S. N. Mohammad and H. Morkoc, “Base transit-time of GaN/InGaN heterojunction bipolar-transistors,” J. Appl. Phys., vol. 78, pp. 4200-4205, Sep. 1995.  W. Lu, L. Wang, S. Gu, D. P. R. Aplin, P. K. L. Yu, and P. M. Asbeck, “InGaN/GaN microwave varactors with high Q, high-breakdown voltage and high linearity,” in IEEE 2011 International Symposium on Semiconductor Device Research (ISDRS), College Park, MD, 7-9 December, 2011.  X. H. Wu, L. M. Brown, D. Kapolnek, S. Keller, B. Keller, S. P. DenBaars, and J. S. Speck, “Defect structure of metal-organic chemical vapor deposition- 88 grown epitaxial (0001) GaN/Al2O3,” J. Appl. Phys., vol. 80, pp. 3228-3237, Sep. 1996.  W. Qian, M. Skowronski, K. Doverspike, L. B. Rowland, and D. K. Gaskill, “Observation of nanopipes in α-GaN Crystals,” J. Cryst. Growth, vol. 151, pp. 396-400, Jun. 1995.  W. Qian, G. S. Rohrer, M. Skowronski, K. Doverspike, L. B. Rowland, and D. K. Gaskill, “Open-core screw dislocations in GaN epilayers observed by scanning force microscopy and high-resolution transmission electron microscopy,” Appl. Phys. Lett., vol. 67, pp. 2284-2286, Oct. 1995.  F. C. Frank, “Capillary equilibria of dislocated crystals,” Acta Crystallogr., vol. 4, pp. 497-501, 1951.  H. Tanaka, Y. Uemura, and Y. Inomata, “Observations of holes around dislocation core in SiC crystal,” J. Cryst. Growth, vol. 53, pp. 630-632, 1981.  H. M. Hobgood, D. L. Barrett, J. P. Mchugh, R. C. Clarke, S. Sriram, A. A. Burk, J. Greggi, C. D. Brandt, R. H. Hopkins, and W. J. Choyke, “Largediameter 6H-SiC for microwave device applications,” J. Cryst. Growth, vol. 137, pp. 181-186, Mar. 1994.  P. G. Neudeck and J. A. Powell, “Performance limiting micropipe defects in silicon-carbide wafers,” IEEE Electron Dev. Lett., vol. 15, pp. 63-65, Feb. 1994.  P. G. Neudeck and C. Fazi, “Positive temperature coefficient of breakdown voltage in 4H-SiC PN junction rectifiers,” IEEE Electron Dev. Lett., vol. 18, pp. 96-98, Mar. 1997.  S. K. Hong, B. J. Kim, H. S. Park, Y. Park, S. Y. Yoon, and Y. I. Kim, “Evaluation of nanopipes in MOCVD grown (0001) GaN/Al2O3 by wet chemical etching,” J. Cryst. Growth, vol. 191, pp. 275-278, Jul. 1998.  Y. Ono, Y. Iyechika, T. Takada, K. Inui, and T. Matsue, “Reduction of etch pit density on GaN by InGaN-strained SQW,” J. Cryst. Growth, vol. 189, pp. 133137, Jun. 1998.  W. Lu, L. Wang, S. Gu, D. P. R. Aplin, D. M. Estrada, P. K. L. Yu, and P. M. Asbeck, “Analysis of reverse leakage current and breakdown voltage in GaN and InGaN/GaN Schottky barriers,” IEEE Trans. Electron Devices, vol. 58, pp. 1986-1994, Jul. 2011. 89  B. Heying, X. H. Wu, S. Keller, Y. Li, D. Kapolnek, B. P. Keller, S. P. DenBaars, and J. S. Speck, “Role of threading dislocation structure on the xray diffraction peak widths in epitaxial GaN films,” Appl. Phys. Lett., vol. 68, pp. 643-645, Jan. 1996.  J. C. Zhang, D. G. Zhao, J. F. Wang, Y. T. Wang, J. Chen, J. P. Liu, and H. Yang, “The influence of AlN buffer layer thickness on the properties of GaN epilayer,” J. Cryst. Growth, vol. 268, pp. 24-29, Jul. 2004.  A. Zubrilov, Properties of Advanced Semiconductor Materials: GaN, AIN, InN, BN, SiC, SiGe (John Wiley & Sons, Inc., New York, 2001).  N. Ohtani, M. Katsuno, T. Fujimoto, T. Aigo, and H. Yashiro, “Surface step model for micropipe formation in SiC,” J. Cryst. Growth, vol. 226, pp. 254260, Jun. 2001.  X. Xu, R. P. Vaudo, J. Flynn, and G. R. Brandes, “Acid etching for accurate determination of dislocation density in GaN,” J. Electron Mater. 31, 402 (2002).  S. K. Hong, T. Yao, B. J. Kim, S. Y. Yoon, and T. I. Kim, “Origin of hexagonal-shaped etch pits formed in (0001) GaN films,” Appl. Phys. Lett., vol. 77, pp. 82-84, Jul. 2000.  X. H. Wu, C. R. Elsass, A. Abare, M. Mack, S. Keller, P. M. Petroff, S. P. DenBaars, J. S. Speck, and S. J. Rosner, “Structural origin of V-defects and correlation with localized excitonic centers in InGaN/GaN multiple quantum wells,” Appl. Phys. Lett., vol. 72, pp. 692-694, Feb. 1998.  Z. L. Miao, T. J. Yu, F. J. Xu, J. Song, C. C. Huang, X. Q. Wang, Z. J. Yang, G. Y. Zhang, X. P. Zhang, D. P. Yu, and B. Shen, “The origin and evolution of V-defects in In(x)Al(1-x)N epilayers grown by metalorganic chemical vapor deposition,” Appl. Phys. Lett., vol. 95, Dec. 2009.  T. Kehagias, G. P. Dimitrakopulos, J. Kioseoglou, H. Kirmse, C. Giesen, M. Heuken, A. Georgakilas, W. Neumann, T. Karakostas, and P. Komninou, “Indium migration paths in V-defects of InAlN grown by metal-organic vapor phase epitaxy,” Appl. Phys. Lett., vol. 95, Aug. 2009.  H. K. Cho, J. Y. Lee, G. M. Yang, and C. S. Kim, “Formation mechanism of V defects in the InGaN/GaN multiple quantum wells grown on GaN layers with low threading dislocation density,” Appl. Phys. Lett., vol. 79, pp. 215-217, Jul. 2001. 90  C. Y. Hsu, W. H. Lan, and Y. S. Wu, “Effect of thermal annealing of Ni/Au ohmic contact on the leakage current of GaN based light emitting diodes,” Appl. Phys. Lett. 83, 2447 (2003).  T. Mizutani, M. Ito, S. Kishimoto, and F. Nakamura, “AlGaN/GaN HEMTs with thin InGaN cap layer for normally off operation,” IEEE Electron Dev. Lett., vol. 28, No. 7, 549-551, 2007.  S. Vitanov, and V. Palankovski, “Normally-off AlGaN/GaN HEMTs with InGaN cap layer: A simulation study,” Solid-State Electronics, 52, 1791-1795, 2008.  T. Palacios, A. Chakraborty, S. Heikman, S. Keller, S. P. DenBaars, and U. K. Mishra, “AlGaN/GaN high electron mobility transistors with InGaN backbarriers,” IEEE Electron Dev. Lett., Vol. 27, No. 1, 13-15, 2006. Chapter 4 Fabrication procedure 4.1 Introduction As we discussed the optimized device structures for achieving high breakdown voltage, high Q and high linearity in chapter 2, an anti-parallel (back-to-back) diode topology with interdigitated structures were employed. For convenience, Figure 2-8 is re-drawn here as Figure 4-1 to show the schematic structure of the designed device. Interdigitated finger dimensions were chosen to be 2.5 m × 2.5 m (finger width × finger spacing), considering the tradeoff between obtaining low series resistance and the limitation of photolithography technique (due to the need to lift-off >1 m-thick metal by photolithography). 91 92 Figure 4-1 Schematic diagram interdigitated strip geometry. 4.2 of the anti-parallel diode structure with Initial fabrication procedure Surface cleaning with NH4OH for native oxide removal and 200-nm Ni thin film deposition by electron beam evaporation were first done immediately after the material MOCVD epitaxial growth to ensure a good interface between semiconductor and metal. 2-inch wafers were then diced into square samples for the following processing. Thick negative photoresist (with a thickness of ~2.4 m after spin coating) was then used to realize the 2.5 m × 2.5 m interdigitated patterns for thick metal lift-off. The metal stack of Ti/Au/Ti/Ni (with a total thickness of ~ 1 m) was then 93 deposited using electron beam evaporation and lifted off by acetone. Next, the wet etch mask for etching the first Ni layer was formed by another photolithography. Ni gate was then patterned by the commercial Ni etchant. A metal sidewall protection layer was then formed by sputtering a 100-nm SiO2 and performing an anisotropic RIE dry etch. The sidewall SiO2 is useful in protecting the Au from being damaged during the following GaN mesa dry etch. Then self-aligned GaN mesa etch to the n+ GaN layer was performed by ICP/RIE etch using BCl3 and Cl2, followed by hot KOH (0.1 mol/L, 90 oC) treatment to remove the etch residuals left after the GaN dry etch. Next, the Ti/Al/Ti/Au ohmic contact was deposited by lift-off process. For device isolation, thick negative photoresist was first pattern by photolithography for hard mask lift-off. SiNx (first) and Ni were deposited by sputtering and electron beam evaporation, respectively, as the hard mask for the following isolation etch (etch ~ 3 m GaN to the insulating c-Sapphire substrate). Ni and SiNx hard masks were then removed by Ni wet etch and SiNx anisotropic dry etch. Benzocyclobutene (BCB) was then spun coat on the sample and cured at 190 oC for 45 mins. Photoresist was then patterned as the mask for the BCB via dry etch. Finally, the Ti/Au pad metal was deposited to contact the underlying metal through the vias for probing and external connections. The schematic diagrams for the varactor fabrication procedure are shown in Figure 4-2. 94 Figure 4-2 Schematic diagrams of the initial GaN-based varactor fabrication procedure. Continued on next page. 95 Figure 4-2 Schematic diagrams of the initial GaN-based varactor fabrication procedure. (a) Epitaxial growth by MOCVD, (b) first Ni deposition, (c) thick metal deposition and first Ni patterning, (d) SiO2 sputtering, (e) SiO2 anisotropic dry etch, (f) self-aligned GaN dry etch, (g) ohmic contact deposition, (h) isolation mask formation, (i) GaN isolation etch to Sapphire substrate, (j) isolation mask removal, (k) BCB spin coating and curing, (l) BCB via etch, (m) pad metal deposition and (n) an optical microscopy image of a finished device. 96 4.3 Preliminary results DC and RF characteristics of the fabricated microwave power varactors were measured. 4.3.1 I-V measurements In order to keep tracking the effects of the device fabrication on the device performance, I-V characteristics of the diodes were taken after every critical fabrication step. Normal forward I-V characteristics were first confirmed by measuring the circular diode Schottky diodes in the sample. Then the reverse I-V characteristics were measured to verify the effects of fabrication step on the reverse leakage current. Two steps in the initial fabrication procedure were found to be detrimental to the device performance. The reverse leakage current was significantly increased after sputtering SiNx (for isolation mask) and curing BCB, as shown in Figure 4-3. The leakage current increase caused by BCB curing is believed to be the defect-related thermal diffusion near the Schottky junction as discussed in section 3.4.4. The leakage current increase caused by sputtering SiNx is likely attributed to the GaN mesa sidewall 97 damage by Ar plasma during the SiNx sputtering. Therefore, high-temperature (>190 o C) process was avoided in subsequent fabrication procedure; a sidewall passivation step should be developed and added after the GaN mesa etch to protect the sidewalls. More detailed work on sidewall passivation will be discussed in the following section. Figure 4-3 Reverse leakage current tracking after critical fabrication steps. (a) Before and after sputtering SiNx and (b) before and after BCB curing. 98 4.3.2 RF measurements The RF measurements were carried out to extract the S-parameters of the devices. The S11 measurement setup is shown in Figure 4-4. The microwave network analyzer HP8753ES is connected to the varactor with a GSG probe. There is a bias Tee in between to protect the network analyzer in case the varactor diodes breakdown at high bias voltages. For the DC path, the device is biased by a voltage source through a DC probe. There is a 50-ohm resistor in parallel with a voltage meter to monitor the reverse leakage current under reverse biases. There is an optional external resistor in case the on-chip n+ GaN serpentine resistor is not high enough in resistance to block the RF signals. Calibration to the GSG probe tips is done using an open/short/load scheme before device measurements. Figure 4-4 Measurement setup for S11. (The measurement data shown below do not necessarily come from the same device structure shown here.) 99 For parameter extractions from the RF measurements, with the varactor considered as a series RC network, the series resistance Rs can be extracted as Rs=Real(Z11); the series capacitance can be extracted as Cs=-1/Imag(Z11); the varactor Q can be extracted as Q=-Imag(Z11)/Real(Z11)=1/(RsCs). A series of measurement results and analysis for a representative anti-parallel diode varactor are shown below. The S11 in the Smith Chart of an anti-parallel diode varactor from 50 MHz to 5.05 GHz at an external reverse bias of 40 V is shown in Figure 4-5. A high Q factor of 104 at 1 GHz, corresponding to a low series resistance of 2.75 was obtained. The Q factor versus frequency f is plotted in Figure 4-6. The roll-off of Q at low frequency is due to RF current flow through the bias network resistors (Rctrl), because the impedance of the varactor is higher at lower frequencies. A Q dip at frequencies near 1.6 GHz is observed. It is also notable that a high Q factor of ~40 was achieved at 5 GHz. 100 Figure 4-5 S11 measured from a device at reverse bias of 40 V from 50 MHz to 5.05 GHz shown in a Smith Chart. It corresponds to Rs=2.75 Ω, Cs=0.56 pF and Q=104. Figure 4-6 Q factor versus frequency at a reverse external bias of 40 V for an antiparallel varactor diode. Each diode has an area of 3.8×10-5 cm2. 101 In Figure 4-7, the reverse leakage current of the measured device was also monitored during the RF measurements by the 50-ohm resistor in parallel with a voltage meter. It is seen that the leakage current becomes significant when reverse bias exceeds 40 V (due to the possible sidewall damage and/or thermal diffusion near the junction as we mentioned in section 4.3.1). In order to fit the experimental curves with simulations and understand the device behavior better, a diode model considering the reverse leakage path is developed. Figure 4-8 shows the simple equivalent circuit model with Rleak, corresponding to the reverse leakage path. Figure 4-7 Reverse I-V characteristics of an anti-parallel varactor diode. 102 Figure 4-8 Equivalent circuit model for the anti-parallel varactors considering Rleak for the reverse leakage current. The extracted series resistance and Q from the measured S11 parameters versus the reverse external bias are shown in Figure 4-9. It should be noted that the reverse external bias is different from the DC control voltage to the anti-parallel diodes due to the voltage drop across the Rctrl (~160 K here) when the leakage current becomes significant. At low biases, Q increases with the reverse external bias due to the reduction in Cs. The low-bias Q can be further improved by thickening the metal stripe. At high bias voltages (>40 V for this device), Q decreases due to the decrease of Rleak (diode is leakier). This can also be seen from the Figure 4-9(a), there is a significant Rs increase when reverse voltage exceeds 40 V where the reverse leakage current starts to become significant. A simple calculation was performed to confirm the relation between Rleak and equivalent Rs (when the parallel Rleak model is converted to the series RC network for Q computation) as shown in Figure 4-10. It is 103 found that the Rs increases as Rleak decreases while the Cs is almost independent with Rleak, Therefore when the device becomes leakier at high biases, there will be a Q drop caused by the decrease of Rleak. This suggests that reducing leakage and maintaining low leakage at high reverse bias are very important for achieving high Q factor as well as high breakdown voltage. Figure 4-9 Extracted series resistance (a) and Q (b) versus reverse external biases for 1 GHz, 2 GHz and 3 GHz. 104 Figure 4-10 and Rleak. Relations between series resistance and Rleak, and series capacitance The extracted capacitance from the S11 measurements versus the effective control voltage Veff=Vdc-Ileak×Rleak (Ileak is the reverse leakage current) is shown in Figure 4-11. The capacitance varies with the effective control voltage as expected. The simulated C-V curve by 1-D Poisson solver fits the experimental curve well. Figure 4-11 Experimental and simulated C-V curves for one of the diode in the two back-to-back diodes. 105 A microwave circuit model based on the equivalent circuit model shown in Figure 4-8 is built using Agilent ADS (a microwave circuit simulator ) to fit the experimental results and understand the RF characteristics of the device. A good match to the experimental results is shown in Figure 4-12. At high frequencies, measured Q values are slightly larger than the model, probably due to parasitic reactance not captured in the model. There is a resonance at ~1.6 GHz in the experimental data, which is believed to be due to a LC resonance and will be addressed in the next chapter. It is worthwhile to show the relation between Q and reverse biases in the simulation when assuming the leakage is low at high reverse biases. A clear trend of Q increase as the increase of reverse bias is shown in Figure 413. This result confirms again the importance of low leakage current to the device performance. 106 Figure 4-12 (a) Experimental Q (dots) and simulated Q (lines) versus the reverse external bias at f = 1 GHz, 2 GHz and 3 GHz; (b) experimental Q (dots) and simulated Q (at reverse external biases of 20 V, 40 V and 60 V) versus frequency. Figure 4-13 Simulated Q versus reverse biases assuming the reverse leakage is low at high biases. 107 4.4 Sidewall passivation in GaN-based Schottky diodes As we discussed in the last sections, the reverse leakage current is important for the device performance and the GaN mesa sidewall damage might be the cause for the increased leakage current after sputtering SiNx for the isolation etch mask. Therefore, a study on the GaN mesa sidewall passivation was carried out. In fact, sidewall passivation is important for power devices. Appropriate sidewall passivation can help reduce leakage current, avoid sidewall damages during later device processing and improve device reliability. This section explores the procedure for the sidewall passivation of GaN-based Schottky diodes by simulation and experiments. 4.4.1 Simulation of electric field distribution under reverse biases In order to understand the importance of sidewall passivation and find the right materials for passivation on GaN sidewalls, simulations using a Silvaco ATLAS 2-D simulator  are performed. The simulated device structure is shown in Figure 4-14. The n- GaN has a doping level of 1×1017 cm-3 and a thickness of 1 m. The structure is almost the same as the structure discussed in section 2.1, except that there is a 108 passivation layer along the sidewall of the GaN mesa. The electric field distributions under reverse biases for various passivation materials with different dielectric constants were simulated. Besides the passivation by growing dielectric materials along the sidewalls, passivation by Mg+ (p-type dopants in GaN) implantation through the sidewall is also simulated. These two types of structure are shown in Figure 4-15. In Figure 4-16(a), it is seen that the simulated electric field at the edge of the Ni-GaN Schottky junction (surrounded by the air) is intensified (~2 MV/cm) and much greater than the electric field in the middle of the junction (~1.7 MV/cm). It suggests that the sidewall (especially the edge) is a great concern for the reverse breakdown and leakage current. The peak electric fields at the edge of the Schottky junctions for didoes with different passivation dielectrics are shown in Figure 4-16(b). It is clearly shown that the peak electric field increases with the relative dielectric constant of the material. The peak electric field of the diode without passivation (in the air) has the lowest intensity compared to those passivated by other relatively high-dielectricconstant materials. The peak electric field of the diode passivated by Mg+ implantation (sidewall surrounded by the air) shows even lower peak electric field at the edge. Although it seems that the intentionally added dielectrics increase the electric field at the edge of the Schottky diodes, it is still necessary to passivate the sidewalls. The reasons are: first, there are likely low-quality passivation materials stick to the sidewalls, e.g. moistures and/or GaOx, when the GaN sidewalls are exposed to the air; secondly, sidewall passivation can physically protect the sidewall from damages during later device processing. Therefore, it will be valuable to conduct a series of experiments to find the appropriate passivation procedure for GaN mesa sidewalls. 109 Figure 4-14 Simulated GaN Schottky diode structure with sidewall passivation in Silvaco ATLAS 2-D simulator for electric field distribution under reverse biases. Figure 4-15 Sidewall passivation by (a) growing dielectrics along the sidewall and (b) Mg+ implantation through the sidewall. 110 Figure 4-16 (a) Electric field distribution under a reverse bias of 85 V and (b) peak electric field at the edge of Ni-GaN Schottky junctions for different passivation materials along the GaN sidewalls. The relative dielectric constants of different materials shown here are from references , . It is also worthwhile to show the electric field distribution for a device with a non-self-aligned gate process (where Ni Schottky gate is not or not aligned to the mask for the GaN mesa etch). The simulated structure and results are shown in Figure 4-17. There is a huge electric field (>7 MV/cm) at the edge of the Ni-GaN Schottky junction (surrounded by air) compared to that (~1.7 MV/cm) in the middle of the junction, which indicates that the non-self-aligned gate structure is not favorable for high power Schottky didoes. 111 Figure 4-17 Electric field distribution for a device with a non-self-aligned gate process. (a) Simulated device structure, (b) electric field distribution near the edge of the Ni-GaN Schottky junction and (c) electric field along the black line (in the red ellipse) in (b) near the edge of the Ni-GaN Schottky junction. 112 4.4.2 Experimental procedure Growth methods used in this study for the passivation dielectrics are atomic layer deposition (ALD) and sputter. Other methods which require high temperature during the growth (e.g. plasma enhanced chemical vapor deposition - PECVD) are excluded in this study due to the possible thermal damages to the Schottky junctions as we discussed in the section 3.4.4. The fabrication procedure is almost the same as described in section 2.1, except that there is additional sidewall treatments after the GaN mesa etch and passivation dielectrics removal (on the Schottky and ohmic contact regions) before ohmic contact deposition. For passivation by dielectric growth, we used sputter at room temperature (RT) for SiO2 (relative dielectric constant = 3.9) passivation and ALD at 175 oC and 210 o C for Al2O3 (= 9) passivation. Before the dielectric deposition, for comparison purpose, hot NH4OH (~60 oC) or KOH (0.1 mol/L, ~80 oC) treatments were used as the chemical treatment to clean the GaN mesa sidewalls after the mesa etch. Measurements in corn oil (= 2.6) immediately after sidewall chemical treatment were also performed. For passivation by Mg+ implantation, the fabrication procedure is schematically summarized in Figure 4-18. Surface treatment with NH4OH and 200-nm Ni e-beam deposition immediately followed the GaN MOCVD growth. The Ni film 113 was then patterned by photolithography and Ni wet etch. A 100-nm SiO2 was sputtered on the surface as the implantation mask (photoresist was left un-removed on top of Ni as additional mask for Schottky junction protection). Two-step Mg+ implantation with ion energy of 60 KeV and 90 KeV (obtained by SRIM simulations  for more uniform implantation profile and sufficient Mg+ implantation at the edge of the Ni-GaN Schottky junction) was then conducted. The implantation dosage was both 1×1014 cm-2 with 90-KeV implantation first. After implantation, the SiO2 mask and residual photoresist on Ni were removed. GaN mesa etch to n+ GaN and hot KOH treatment were then performed. Finally, ohmic contact deposition on the n+ GaN was done to finish the device fabrication. The schematic device structures for these two passivation methods are shown in Figure 4-15, except that the ohmic contacts are not shown. 114 Figure 4-18 Fabrication procedure for sidewall passivation by Mg+ implantation. (a) Ni patterning by wet etch, (b) SiO2 sputtering for implantation mask, (c) Mg+ implantation and (d) SiO2 and photoresist removal, GaN mesa etch and ohmic contact deposition. 4.4.3 Results and discussions GaN Schottky diodes fabricated with different sidewall processing procedures were labeled accordingly in Table 4-1. 115 Table 4-1 methods. Samples treated with different sidewall cleaning and passivation Sample labels Chemical treatment Sidewall passivation Control KOH No NH4OH_Oil NH4OH Oil KOH_Oil KOH Oil KOH_ALD_Al2O3_175C KOH ALD Al2O3 at 175 oC NH4OH_ALD_Al2O3_210C NH4OH ALD Al2O3 at 210 oC KOH_ALD_Al2O3_210C KOH ALD Al2O3 at 210 oC KOH_Sput_SiO2 KOH Sputter SiO2 at RT KOH_Mg_Imp KOH Mg implantation The reverse I-V measurement results for all samples listed above are summarized in Figure 4-19. It is seen that hot KOH treatment is effective in cleaning GaN sidewall (possible GaN residuals caused by GaN mesa etch and/or GaOx) before the passivation. After treated with hot KOH, dielectric passivation of corn oil and 175o C-ALD Al2O3 (sample KOH_Oil and KOH_ALD_Al2O3_175C) as well the passivation by Mg+ implantation (sample KOH_Mg_Imp) work well as GaN sidewall passivation layers, showing significant reverse leakage current reduction in comparison with the Control sample. However, hot NH4OH treatment seems to damage the GaN sidewalls (forming more sidewall states by physical and/or chemical damages) and cause excess leakage current, which can be observed from reverse I-V characteristics of the sample NH4OH_Oil and NH4OH_ALD_AL2O3_210C. These 116 observations confirm that appropriate sidewall passivation is a necessary for fabricating GaN-base power Schottky diodes in order to protect the sidewall from being damaged by other device processing. The sample passivated by 210 oC-ALD Al2O3 showed excess leakage current too which is due to the thermal damage to the Ni-GaN Schottky junctions as discussed in section 3.4.4. For sidewall passivation by SiO2 sputtering, the diode became very leakage too which we believe was caused by the sidewall damage due to the Ar plasma during the SiO2 sputtering. In comparison, ALD is a more gentle growth technique which does not cause damage to the materials. Figure 4-19 Reverse leakage current for samples fabricated with different sidewall processing procedures. The diode area is 2.8×10-5 cm2. 117 4.4.4 Summary of sidewall passivation in GaN-based Schottky diodes The importance of sidewall passivation in GaN-based power Schottky diodes was confirmed by simulations and experiments. In the simulations, we found that the electric field at the edge of Ni-GaN Schottky junctions under reverse biases was much greater than that in the middle of the junctions (due to geometric effect). It brings forth a concern of the mesa sidewalls for GaN-based Schottky diodes in high power applications. Experimentally, we tried different chemical treatments before sidewall passivation for sidewall cleaning as well as different sidewall passivation methods. KOH was found to be effective in cleaning GaN sidewalls and low-temperature-ALD Al2O3 and Mg+ implantation were effective in passivating the sidewalls. 4.5 Improved fabrication procedure The fabrication procedure is therefore adjusted based on our experiments and analysis. The main improvements are as follows: the interdigitated finger stripe 118 thickness is increased up to >1.8 m by improving the photolithography and lift-off technique; a hot KOH treatment after the GaN mesa etch followed by an immediate ALD Al2O3 sidewall passivation at 170 oC are added; BCB curing temperature is lowered to 170 oC. (The reason for selecting low-temperature ALD Al2O3 instead of Mg+ implantation is due to the equipment availability at UCSD). The adjusted fabrication steps and the resultant reverse I-V characteristics after the ohmic metal was formed and after all of the device processing were finished are shown in Figure 4-20. In comparison to the reverse I-V characteristics shown in Figure 4-3, the leakage current is greatly reduced and maintained at low levels after finishing the device fabrication. The RF measurements and the detailed analysis for the devices fabricated with the improved procedure will be discussed in the next chapter. 119 Figure 4-20 Improved fabrication procedure and the resultant reverse I-V characteristics. (a) Thick (> 1.8 m) metal deposition and lift-off, (b) hot KOH treatment and ALD Al2O3 passivation at 170 oC for GaN mesa sidewalls, (c) low temperature (170 oC) BCB curing and (d) reverse I-V curves after the ohmic metal was formed (the I-V characteristics can be measured from now) and after all device fabrication was finished. The measured diode in (d) is a circular diode with diameter of 60 m. 4.6 Summary of the fabrication procedure The initial fabrication procedure is described in this chapter. DC and RF characterization were performed to extract the preliminary characteristics of the fabricated microwave power varactors. A high Q = 104 at 1GHz was obtained at a 120 reverse bias of 40 V. However, excess leakage current was found in the devices possibly due to the GaN mesa sidewall damage caused by Ar plasma during the SiNx sputtering and the Schottky junction degradation caused by the defect-related thermal diffusion during BCB curing. Simulations and experiments were then carried out to improve the fabrication procedure. Hot KOH treatment after GaN mesa etch, lowtemperature ALD Al2O3 (as well as Mg+ implantation) sidewall passivation and lowtemperature BCB curing were found to be effective in maintaining low leakage current throughout the entire fabrication process. Section 4.3, is a rearrangement of the paper “InGaN/GaN Microwave Varactors with High Q, High-Breakdown Voltage and High Linearity,” Wei Lu, Lingquan (Dennis) Wang, Siyuan Gu, David P. R. Aplin, Paul K. L. Yu, and Peter M. Asbeck, in Semiconductor Device Research Symposium (ISDRS), 2011 International, IEEE, College Park, MD, 7-9 Dec., 2011. The dissertation author was the primary author of the paper. 121 4.7 References  http://edocs.soco.agilent.com/display/ads2009/Home  http://www.silvaco.com/products/device_simulation/atlas.html  J. Robertson, “High dielectric constant oxides,” Eur. Phys. J. Appl. Phys., vol. 28, 265-291, 2004.  M. Passlack, N. E. J. Hunt, E. F. Schubert, G. J. Zydzik, M. Hong, J. P. Mannaerts, R. L. Opila, and R. J. Fischer, “Dielectric properties of electronbeam deposited Ga2O3 films,” Appl. Phys. Lett., vol. 64, No. 20, 2715-2717, 1994.  http://www.srim.org/ Chapter 5 Experimental results and discussions Complete characterization of the GaN-based microwave power varactors was carried out and the results are presented in this chapter, including high voltage C-V and I-V measurements, S-parameter measurements, linearity measurements and tunable resonance circuit measurements. 5.1 High voltage I-V and C-V measurements The forward I-V characteristics were first measured on the circular diodes in the sample as shown in Figure 5-1. The extracted ideality factor and Schottky barrier height are 1.24 and 1.25 eV, respectively. 122 123 Figure 5-1 sample. Forward I-V characteristics for a 60-m-diameter circular diode in the In Figure 5-2, the reverse I-V characteristics show a breakdown voltage of above 100 V and much lower leakage current for the device fabricated using the improved fabrication procedure than those fabricated using the initial fabrication procedure (refer to Figure 4-3). Figure 5-2 sample. Reverse I-V characteristics for a 60-m-diameter circular diode in the 124 The high voltage C-V characteristics for a single circular diode varactor were then measured as shown in Figure 5-3(a). The capacitance varies with the reverse applied biases up to 100 V. The measured C-V curve is consistent with the simulated curve except that the last several points of the measured C–V curve are lower due to the large leakage current when the reverse bias approaches 100 V, which causes the unreliability of the capacitance measurement. Base on the measured high-voltage C-V curve, we then worked out the corresponding tuning ratio (Cmax/Cmin) of an antiparallel diode varactor as shown in Figure 5-3(b). The tuning ratio is calculated based on the considerations that the summation of the DC and RF signal to the diodes does not cause any reverse breakdown or forward conduction. It is noted that a tuning ratio of 2 is still maintained for a RF peak-to-peak voltage of ~80 V. 125 Figure 5-3 (a) High voltage C-V characteristics for a circular diode with an area of 5×10-5 cm2 at f = 1 MHz and (b) the corresponding tuning ratio vs RF peak-to-peak voltage for the anti-parallel diode varactor, based on the considerations of not causing reverse breakdown or forward conduction. The waves shown in (a) denote the RF signals at the minimum and maximum DC bias voltages when calculating the tuning ratio. 5.2 S-parameter measurements 126 The RF characteristics of the microwave varactors were obtained via two measurement layouts for 1-port and 2-port measurements, respectively. Two representative microwave varactors under the optical microscopy and their corresponding equivalent LRC network are shown in Figure 5-4. Figure 5-4(a) shows the device for 1-port measurements, which have the ~1.8-m-thick metal stripe and 2.5 m × 2.5 m interdigitated finger structures, same as the design we discussed in chapter 4. The 2-port device shown in Figure 5-4(b) has slightly different interdigitated structures. The fingers have a length of 120 m, a width of 7 m (50 m and 2.5 m, respectively, for the narrower finger design shown in Figure 5-4(a)) and a spacing of 2.5 m between fingers. The reasons for the wider and longer finger design are to increase the capacitance density (per finger) and further thicken the finger metal stripe utilizing the final pad metal deposition (vias can be fully opened along the fingers when the fingers are wide enough). 127 Figure 5-4 (a) An optical microscopy image of a device for 1-port measurements, (b) an optical microscopy image of a device for 2-port measurements, (c) the equivalent series LRC network for the 1-port device and (d) the equivalent series LRC network for the 2-port device. The parameter extraction formulas for the equivalent series LRC network are as follows: For 1-port measurements: ( ( ( ) ), ( ) ), ( ) ( ) ( ). Eq. 5-1 For 2-port measurements: 128 ( ( ( ) ), ( ) ), ( ) ( ) ( ). Eq. 5-2 The series inductance can be measured from a short de-embedding structure, which is usually a small value in the order of 0.1 nH. However, the extracted Cs and Q(w) shown in the follow sections did not subtract the jwLs term, which gives a lower but more accurate Q values for the devices. 5.2.1 Measurements for the 1-port devices The anti-parallel diode varactor devices for 1-port measurements were measured up to a reverse bias of 70 V. The measurement setup is the same as the one shown in Figure 4-4. The reserve leakage current was recorded from the 50-ohm resistor in parallel with a voltage meter, as shown in Figure 5-5. The leakage current is much lower than that of the previous device fabricated with the initial fabrication procedure. 129 Figure 5-5 Reverse I-V curve for a 1-port anti-parallel diode varactor (see Figure 5-4(a)). The dots are the measurement data points. Figure 5-6 shows the measured S11 in the Smith Chart from 500 MHz to 3.5 GHz for the same 1-port device at a reverse bias of 70 V. At 1 GHz, it corresponds to a capacitance of 0.55 pF, a series resistance of 2.4 Ω. Correspondingly, a high Q of 120 was obtained at 70 V for the fabricated 1-port device with the improved fabrication procedure. Figure 5-6 70 V. S11 from 500 MHz to 3.5 GHz for a 1-port device at a reverse bias of 130 The relations of Q versus reverse bias, Rs versus reverse bias and Cs versus reverse bias are shown in Figure 5-7. In comparison with the same relations for a leakier device fabricated using the initial fabrication procedure shown in Figure 4-9, the Q does not drop in value at high reverse bias for the new devices (Rs does not jump up too much at high reverse biases either). Another improvement is that the Q at low biases (~90 at 1 GHz) is much larger than the previous results (~50 at 1 GHz) obtained from the device with the same structure. This is attributed to the thicker metal stripes which are almost doubled in thickness in the improved fabrication procedure. Figure 5-7(c) shows the C-V curves extracted from the S11 measurements. Although the capacitance decreases with the increase of the reverse bias, the curve cannot be fitted with the calculated C-V curve by running a simple 1-D Poisson simulation. This is probably due to some parasitic reactance and/or imperfection of the device fabrication which are not captured in the equivalent circuit model. More analysis will be discussed in the next section. 131 Figure 5-7 The relations of (a) Q versus reverse bias, (b) Rs versus reverse bias and (c) Cs versus reverse bias at 1 GHz, 2 GHz and 3 GHz for a 1-port device. 132 Figure 5-8 shows the relation between Q and frequency at different reverse biases. Q of above 100 (up to 120) at 1 GHz and above 50 at 3 GHz are obtained. Different from our expectation, the Q did not show the anticipated strong dependence on reverse biases, probably due to the effects of parasitic reactance in the device. Several resonances in the Q versus frequency curves are also observed at frequencies between 1 GHz and 2 GHz, which are believed to be attributed to the LC resonance in the DC path and confirmed by the following simulations. Figure 5-8 port device. The relation of Q versus frequency at different reverse biases for a 1- As shown in Figure 5-9, a more detailed equivalent circuit model incorporating the parasitics from the device and measurement setup is simulated in ADS. In comparison with the simple model shown in Figure 4-8, the inductance from the DC needle probe (~1 nH/mm) and the coaxial cables (~ 300 nH/m for RG-58/U) in the DC 133 path is very large (770 nH used in this simulation, 750 nH from the coaxial cable and 20 nH from the DC needle probe) and cannot be subtracted in the RF calibration using a standard open/short/load calibration substrate. The parasitic capacitance (0.01 pF used in this simulation and confirmed by a SONNET electromagnetic simulation ) of the n+ GaN control resistor is also included in this model. The stray capacitance shown in the model is mainly from the capacitance between fingers. The small capacitance to the ground is also included in this model. Figure 5-9 Equivalent circuit model considering the parasitics from the 1-port device and the measurement setup. The simulation results based on the above model showed very good match with the experimental results as shown in Figure 5-10(a) (only match one of the resonances though). The LC resonance between the inductor from the DC probe and 134 coaxial cable (770 nH) and the capacitance from the n+ GaN resistor (0.01 pF) caused a Q dip. This is due to the RF leak through the DC path at the resonant frequency (low impedance in the DC path). In practical package, the inductance from the DC path should be much smaller so that a resonance will be expected at a much higher frequency. The simulated Q vs frequency assuming the inductance in the DC path is small (10 nH) is also shown in Figure 5-10(b). No Q dip is observed in the simulated frequency range. Similar to the Q versus frequency curve shown before in Figure 4-12, the Q is also higher than the simulated values at higher frequencies in Figure 5-10, which is probably due to some parasitic reactance not captured in the circuit model. 135 Figure 5-10 Experimental and simulated Q versus frequency curves at different reverse biases for a 1-port device. (a) The simulation considers the LC resonance in the DC path and (b) the simulation (dashed curves) does not consider the LC resonance in the DC path. 136 5.2.2 Measurements for the 2-port devices The schematic diagram for the 2-port measurements is shown in Figure 5-11. Calibration to the two GSG probe tips using an open/short/load/through scheme was done before device measurements. Same as the 1-port measurement setup, there are bias-Tees in between the network analyzer and the GSG probe tips to protect the network analyzer at high reverse biases; the leakage current is recorded during the measurements through a 50-ohm resistor in parallel with a voltage meter. Figure 5-11 Schematic diagram for the 2-port measurements. 137 The improved reverse I-V characteristics by using the improved fabrication procedure are first shown in Figure 5-12. The leakage is slightly higher than the 1-port device shown above due to a larger diode area. Figure 5-12 Reverse I-V curve for a 2-port anti-parallel diode varactor. The dots are the measurement data points. The representative S-parameters from 500 MHz to 3.5 GHz for the varactor 2port measurements are shown in Figure 5-13. The S11 in the Smith Chart goes from the open (high reflection) to the 50 ohms (low reflection) along the 50-ohm resistance circle from low frequency to high frequency, indicating a capacitor with a lowresistance series resistor from the device; the magnitude of S21 (along the 50-ohm resistance circle as well) increases with the frequency increase, indicating higher transmission at higher frequencies (due to the lower impedance from the device at higher frequencies). 138 Figure 5-13 The representative S-parameters for the varactor 2-port measurements. The relations of Q versus reverse bias, Rs versus reverse bias and Cs versus reverse bias are shown in Figure 5-14. The clear trends of Q increase and Rs decrease at 1 GHz with the increase in reverse biases are shown in Figure 5-14(a) and 5-14(b), respectively. This trend is consistent with the theoretical expectation: when reverse bias increases the depletion thickness in n- GaN increases as well, which results in a lower Cs and Rs so that a higher Q. A high Q of >180 was thus achieved at 1 GHz. However, the trends for the data at 2 GHz and 3 GHz are not as clear as the data at 1 GHz, possibly due to the parasitic reactance from the device. Figure 5-14(c) shows the C-V curves extracted from the 2-port S-parameter measurements. The simulated C-V curve using a 1-D Poisson solver fit the experimental results very well. It indicates that the layout of the 2-port devices suffers much less parasitic components. In comparison with the C-V curves obtained from the 1-port devices shown in Figure 5-15, the 139 mismatch between the experimental results and theoretical simulations for the 1-port device is likely due to more parasitics and/or more processing errors during the fabrication for the narrower and shorter interdigitated finger structures. For example, a 0.25 m undercut during the Ni wet etch represents 20% error for the 2.5-m-wide fingers but only 7% for the 7-m-wide fingers. The Ni undercut certainly reduces the actual area of the Schottky contact (the measured capacitance is lower than the simulated capacitance at zero bias as shown in the Figure 5-15) and changes the electric field distribution underlying the Schottky contact so that the C-V characteristics of the varactor diodes as well. 140 Figure 5-14 The relations of (a) Q versus reverse bias, (b) Rs versus reverse bias and (c) Cs versus reverse bias at 1 GHz, 2 GHz and 3 GHz for a 2-port device. 141 Figure 5-15 port device. The experimental and simulated Cs versus reverse bias curves for a 1- The relation of Q versus frequency extracted from the S-parameter measurement is then shown in Figure 5-16. A Q of above 70 at 2 GHz was obtained. Unlike the measurements done on the 1-port device, the Q shows a strong dependence on reverse biases which is consistent with the theoretical prediction. Several resonances in the Q versus frequency curves are also observed at frequencies between 1 GHz and 2 GHz, which are attributed to the LC resonance in the DC path, same as the 1-port measurements. 142 Figure 5-16 The relation between Q and frequency at different reverse biases for a 2-port device. The ADS simulation results based on the same model shown in Figure 5-9, except that there is a port 2 symmetrically located at the other side of the varactor diode as the RF output, are shown in Figure 5-17. The inductance from the DC needle probe and the coaxial cable and the capacitance from the n+ GaN resistor are identical with the values used in the 1-port simulations. The simulated curves fit the experimental curves reasonably well including the LC resonances from the DC path (only match one of the resonances though). The simulated curves without considering the LC resonance from the DC path are also included in the Figure 5-17(b). 143 Figure 5-17 Experimental and simulated Q versus frequency curves at different reverse biases for a 2-port device. (a) The simulation considers the LC resonance in the DC path and (b) the simulation (dashed curves) does not consider the LC resonance in the DC path. More 2-port devices with different areas and structures were also measured. Their optical microscopy images and the corresponding Q versus frequency curves (including the one discussed above) are shown in Figure 5-18. As theoretically 144 expected, a clear trend of Q increase with the increase of reverse bias is observed for all of the 2-port devices. In comparison, the Q does not show clear dependence on the reverse biases for the 1-port devices. It is also shown that the Q is higher for smaller devices: Q > 250 at 2 GHz was obtained for varactors with Cmax (when reverse bias is zero) less than 1 pF. However, the high Q values at the low frequencies are not reliable because of LC resonance in the DC path. This unrealistically high Q values become more obvious for the very small device, e.g., the device shown in Figure 518(c). That is because when the capacitance of the varactor is low, the impedance of the varactor becomes high so that the RF signal leaks more through the DC path, especially near the LC resonance frequencies. 145 Figure 5-18 Optical microscopy images and the corresponding experimental Q versus frequency curves for the 2-port devices with different areas and structures. Cmax corresponds to the capacitance of the varactor at zero reverse bias. 146 5.3 Linearity measurements The linearity property of microwave power varactors was evaluated via a twotone test and an experiment using a 2-W WCDMA signal input. 5.3.1 Two-tone test The two-tone test measurement setup is shown in Figure 5-19. Power amplifiers are used after the two signal generators to increase the input power in order to obtain the measureable IM3 (third-order intermodulation) above the noise floor of the spectrum analyzer. Attenuators (not shown in the diagram) are used before the spectrum analyzer to minimize the IM3 generated from the spectrum analyzer. The anti-parallel diode varactor is connected in shunt to a 50- line (spectrum analyzer). The frequencies of the two tones are 1.1 GHz and 1.115 GHz, respectively. Before the two-tone test for the varactors, the linearity of the measurement setup was first verified by measuring the OIP3 (third-order intercept point) without having the varactors in the measurement circuit. 147 Figure 5-19 Measurement setup for the two-tone test. As shown in Figure 5-20, at RF input power of 26 dBm to the measured varactor, the IM3 products were at a level of -90 dBc relative to the outputs at the input frequencies (for a control reverse bias voltage of 25 V). This corresponds to an OIP3 of 71 dBm. However, equipment limitations prevented obtaining accurate IM3 values for larger reverse biases (where much higher OIP3 values are expected): IM3 is buried under the noise floor of the spectrum analyzer. By contrast, for single varactor diodes, the measured OIP3 value was 36 dBm, for control voltage set to 0 V, showing much worse linearity. 148 Figure 5-20 Output power at fundamental and IM3 frequencies versus the input power for an anti-parallel diode varactor (1-port) at a control reverse bias of 25 V. The reverse voltage dependence of a single diode varactor can be usually expressed as ( ) ( ) Eq. 5-3 where K is the capacitance constant, is the built-in potential of the diode, V is the reverse voltage and n is the exponent of the voltage dependence of the diode capacitance. The linearity of the anti-parallel diode has a strong dependence on the n factor. Theoretically a distortion-free varactor diode can be achieved with n = 0.5, which corresponding to a Schottky diode with uniform doping . An ADS simulation, assuming the varactor follows the C-V characteristics as Eq. 5-3, was performed to verify the OIP3 of the device. The n factor for the device (1-port) we 149 measured is 0.4, confirmed by the C-V curve fitting, although the doping in the varactor region is uniform. The deviation of the extracted n factor (< 0.5) is probably caused by the parasitic components in the device and/or the imperfection of the device fabrication (e.g., the formation of the Ni undercut during Ni wet etch). The experimental and simulated results including the ideal case of n = 0.5 are shown in the Table 5-1. The simulated OIP3 of 73 for the measured 1-port device (n = 0.4) at a reverse bias of 25 V is almost consistent with the measured value. The simulated OIP3 of 80.5 at a reverse bias of 25 V for the ideal case (n = 0.5) indicates that a much higher OIP3 can be obtained by further improving the device layout and fabrication procedure. A minimum OIP3 requirement in the wireless base station applications is also listed in the table. It suggests that the obtained OIP3 for our varactors already meets the linearity requirement in some practical applications. Table 5-1 Measured and simulated OIP3 for the anti-parallel diode varactor with different n factors. n Meas_OIP3 (dBm) at 25V Simu_OIP3 (dBm) at 25V 0.4 70 73 0.5 N.A. 80.5 OIP3 requirement in wireless base-station applications (dBm) >65 150 5.3.2 2-W WCDMA signal input The linearity of the varactor was also evaluated by using a 2-W WCDMA signal input experiment. The measurement setup is shown in Figure 5-21. The linearity of the system was first calibrated by measuring without the varactor in the measurement setup. The maximum average power that the WCDMA signal generator can output without significant signal distortion (nonlinearity) is ~-17 dBm. The peak to average ratio (PAR) of this WCDMA signal is 7.8 dB. The power amplifier has a gain of 50 dB. Therefore, the maximum average and peak power (without significant signal distortion from the system) of the WCDMA input signal to the varactor are 33 dBm and 40.8 dBm (2 W and 12 W), respectively. Figure 5-21 Measurement setup for the WCDMA signal input experiment. The measured adjacent channel leakage ratio (ACLR) for a small 1-port device with a WCDMA signal input of 2 W (12 W peak power) is -53 dBc as shown in 151 Figure 5-22. It indicates that the IM3 is still negligible under such high input power levels. Figure 5-22 Adjacent channel leakage ratio (ACLR) for a small 1-port device with a 2-W (12-W peak power) WCDMA signal input. A simulation was carried out to calculate the actual RF voltage (corresponding to the actual RF power) applied to the varactor diode. Figure 5-23(a) shows the equivalent circuit model of the measurement system. The RF cables were considered as transmission lines for more accurate simulations. As seen in Figure 5-23(b), the RF voltage applied to the varactor (named Vcap in the simulation) is almost identical to the RF voltage coming from the signal generator (named Vsc in the simulation). This simulation results confirmed the validity of the measurement system so that the measurement result: the anti-parallel diode varactor with a low ACLR of <-53 dBc under a 2-W (12-W peak power) WCDMA signal input has been achieved. 152 Figure 5-23 (a) Equivalent circuit model of the measurement system for the WCDMA signal input experiment, and (b) simulated instantaneous RF voltage at different nodes. 5.4 Application in the tunable resonant circuit 153 The preliminary application of the varactor is demonstrated by building a tunable resonant circuit using the varactor and transmission lines. The measurement setup up is shown in Figure 5-24. Figure 5-24 Measurement setup of the tunable resonant circuit using the varactor and transmission lines. The resonance mainly comes from the varactor and the series transmission line. Different length of transmission lines (for the transmission line that is in series with the varactor) were used to see the resonance at different frequencies. Figure 5-25 shows the well matched measurement and simulation results with the seriestransmission-line length of ~7 cm and ~11 cm. 154 Figure 5-25 (a), (b) Experimental and (c), (d) the corresponding simulated S21 curves from 0.5 GHz to 2.5 GHz, for the tunable resonant circuit using varactor and transmission lines. (a) uses a shorter (~7 cm) transmission line in series with the varactor and (b) uses a longer (~11 cm) one. Different resonance frequencies were observed for the resonance circuits using different length of the series transmission lines. It is also seen that the resonance frequency varies with the control bias voltage of the varactor. These results suggest that these varactors are already good for designing sharp tunable filters. 155 5.5 Summary This chapter reported the experimental DC and RF measurement results and the corresponding analysis for the GaN-based microwave power varactors fabricated with the improved fabrication procedure. Benefited from the improved fabrication procedure (better reverse I-V characteristics, thicker metal stripe thickness, etc.), the breakdown voltage of greater than 100 V, Q of above 120 at 1 GHz for 1-port device and Q of above 250 at 2 GHz for small 2-port devices, and OIP3 of >71 dBm (ACLR of <-53 dBc under 2-W WCDMA signal input) were obtained. Real applications in the tunable resonant circuit were also demonstrated. The results indicate that the varactors already meet the representative requirements for some practical use. 156 5.6 References  http://www.sonnetsoftware.com/  K. Buisman, L. C. N. de Vreede, L. E. Larson, M. Spirito, A. Akhnoukh, T. L. M. Scholtes, and L. K. Nanver, “Distortion-free varactor diode topologies for RF adaptivity,” in Proc. IEEE MTTS Int. Microwave Symp., Long Beach, CA, pp. 157–160, Jun. 2005. Chapter 6 Conclusion and Future Work The goal of this study was to develop material and device structures for high power, high Q and high linearity microwave varactors for the wireless base station applications. The detailed results demonstrated in this work potentially meet the specifications for practical use. However, more work is still needed in order to achieve better performance and possibly commercialization. 6.1 Summary of the thesis This dissertation presented the design, fabrication and characterization of GaNbased microwave power varactors. The results and conclusion are summarized below: 1) The design rules for high power, high Q and high linearity microwave varactors have been developed. GaN, with its high electron mobility and high breakdown electric field, showed the highest figure-of-merit Qmin in 157 158 comparison with other common semiconductors, is therefore considered a prime candidate material. 2) InGaN surface layer has been designed to increase the breakdown voltage and reduce the reverse leakage current for GaN-based Schottky diodes. Experimentally, the breakdown voltage of the GaN-based Schottky diodes was increased to >120 V from ~80 V by employing the InGaN surface layer design. 3) Comprehensive studies on the Ni-InGaN/GaN Schottky barriers (using InGaN surface layer design) were carried out. Due to the polarization induced charges at the InGaN/GaN interface, the electron tunneling probability of InGaN/GaN Schottky barrier is greatly suppressed in comparison with the GaN-only design. As a result, the reverse leakage current and breakdown voltage of the InGaN/GaN Schottky diodes are improved. The polarization chargers at the InGaN/GaN interface influence the forward I-V characteristics of the InGaN/GaN Schottky diodes as well: a subthreshold slope of > 60 mV/decade is caused by the forward bias dependent Schottky barrier height (induced by the polarization charges at the interface). These forward and reverse I-V characteristics are different from those of the GaN-only design as confirmed by experimental measurements and theoretical simulations. The HP-MOCVDgrowth technique of the GaN buffer layer was also found to be effective in reducing the leakage current and increasing the breakdown voltage of GaN Schottky barriers by achieving low-defect-density materials. Surface 159 micromesas were observed on InGaN/GaN epi-layers by NOM, SEM and AFM, mostly originated from nanopipes in GaN. Studies of RBS and the electrical characteristics on corresponding Ni-InGaN/GaN Schottky barriers indicated that the surface micromesas with nanopipes at the center were the main source of reverse leakage current and introduced an easy metal diffusion path, even under relatively low-temperature thermal anneal. The application of InGaN surface layer design in the enhancement-mode GaN-based HEMTs was also introduced. 4) An initial fabrication procedure was first developed. The DC and RF measurements performed on the devices fabricated using the initial fabrication procedure indicated that the device performance (Q, reliability, etc.) suffered from excess reverse leakage current which was caused by certain fabrication steps. Sidewall damage and defect-related thermal diffusion near the Ni-InGaN junction were found to be the reasons for the excess leakage caused during the device fabrication. An improved fabrication procedure was successfully developed. Avoiding any high temperature processing (> 190 oC) and ALD Al2O3 with KOH pre-treatment for GaN mesa sidewall passivation were found to be important in reducing leakage current and maintaining low leakage current during the device fabrication. 5) Benefited from the improved fabrication procedure, the reverse leakage current was maintained at low levels after the entire device fabrication. DC and RF 160 characterizations have confirmed high performance GaN-based microwave power varactors. The breakdown voltage of greater than 100 V, Q of above 120 at 1 GHz for 1-port device and Q of above 250 at 2 GHz for small 2-port devices, and OIP3 of >71 dBm (ACLR of <-53 dBc under 2-W WCDMA signal input) were obtained. The real application in the tunable resonant circuit was also demonstrated. The results indicate that the varactors already meet the representative requirements for some practical use. 6.2 Comparison of different varactor technologies The performance parameters of different varactor technologies are summarized in Table 6-1. GaAs, Si-on-glass and MEMS varactor technologies can achieve very high Q at high frequencies, however, are usually used in low power levels. The Q would be expected to be significantly lower when these technologies are used for high operation voltages as we discussed in Chapter 1. Specifically for MEMS technology, it achieved a Q of > 80 at 40 GHz and breakdown voltage of > 34 V. However, due to its mechanical operation, the switching speed is slow (typically in MHz range) in comparison with the Schottky diode technology. The reliability is also a concern for the mechanical system (mechanical parts are prone to damage after certain number of operations). 161 For high power varactors, recently high-voltage and high-Q SiC microwave varactors have been reported. A Q of 160 at 2 GHz with breakdown voltage of >150 V was achieved. However, the reported SiC varactor was based on a single diode structure and the linearity of the device has not been reported yet. In our work, a Q of > 70 at 2 GHz with breakdown voltage of > 120 V for a large diode (with C max = 1.8 pF for an anti-parallel diode varactor in comparison with the Cmax = 0.9 pF reported for the SiC single diode varactor). For smaller varactors, a much higher Q of above 250 at 2 GHz has been achieved. For the linearity, by employing the anti-parallel diode device topology, an OIP3 of >71 dBm and an ACLR of <-53 dBc under a 2-W WCDMA signal input were obtained. To the best of our knowledge, GaN-based microwave power varactors currently show the best performance in terms of the combination of breakdown voltage, Q and linearity properties. Table 6-1 The performance parameters of different varactor technologies. Technology Q Breakdown (V) OIP3 (dBm) GaAs (2 GHz)  62 (max) 28 57 Si-on-glass (2 GHz)  100~300 >12 60 MEMS (40 GHz)  >80 >34 N.A. 160 (max) >150 N.A. >70 (max) >120 70 SiC (2GHz, C =0.9 pF)  max This work (GaN at 2GHz, C =1.8 pF) max 162 6.3 Future work In retrospect, there are a few areas of further investigation for advancing the GaN-based high power microwave varactors that employ Schottky barriers: 1) From the fabrication point of view, it is important to further improve the fabrication procedure to maintain low leakage current and high breakdown voltage during the device fabrication. This not only affects the Q factor but also the reliability of the device. Additionally, as discussed in section 5.2, Ni undercut formed by the Ni wet etch is a problem, especially for the narrower finger devices, causing non-ideal C-V tuning and possible nonlinearity to the anti-parallel diode varactors (due to the resultant n ≠ 0.5 in Eq. 5-3). Therefore, improving the fabrication procedure to mitigate the Ni undercut is important for obtaining better performance. A straightforward method is to decrease the thickness of the first Ni layer (which is in contact with the semiconductor), in which less etch time is needed so that less undercut can be achieved. Another possible way to further improve the Q factor is to further increase the metal stripe thickness to achieve lower series resistance. 163 2) From the analysis point of view, it is important to further explore the reasons responsible for different characteristics of the 1-port and 2-port devices, although some analysis has been made in chapter 5. This can be valuable for the future device designs. 3) The LC resonance in the DC path should be considered in the future device/circuit designs. As for avoiding the LC resonance in the measurements, a big series inductor can be added into the DC path. 4) Demonstrate other circuit applications, e.g., tunable filters, high-efficiency, high power, tunable power amplifiers. 164 6.4 References  C. Huang, P. J. Zampardi, K. Buisman, C. Cismaru, M. Sun, K. Stevens, J. Fu, M. Marchetti, and L. C. N. de Vreede, “A GaAs junction varactor with a continuously tunable range of 9:1 and an OIP3 of 57 dBm,” IEEE Electron Device Lett., vol. 31, no. 2, pp. 108–110, Feb. 2010.  C. Huang, K. Buisman, M.Marchetti, L. K. Nanver, F. Sarubbi, M. Popadi´c, T. L.M. Scholtes, H. Schellevis, L. E. Larson, and L. C. N. de Vreede, “Ultra linear low-loss varactor diode conﬁgurations for adaptive RF system,” IEEE Trans. Microw. Theory Tech., vol. 57, no. 1, pp. 205–215, Jan. 2009.  J. S. Fu, X. A. Zhu, J. D. Phillips, and A. Mortazawi, “Improving linearity of ferroelectric-based microwave tunable circuits,” IEEE Trans. Microw. Theory Tech., vol. 55, no. 2, pp. 354–360, Feb. 2007.  C. M. Andersson, N. Ejebjörk, A. Henry, S. Andersson, E. Janzén, H. Zirath, and N.Rorsman, “A SiC Varactor With Large Effective Tuning Range for Microwave Power Applications,” IEEE Electron Device Lett.,vol. 32, no. 6, pp. 788–790, Jun. 2011. Appendix A GaN-based varactor fabrication procedure Part I: Schottky contact and thick metal deposition 1. Grow material using MOCVD. 2. Immediately immerse wafer into NH4OH for 1min (without DI water rinse) and dry with N2 blow. 3. Immediately deposit Ni (Schottky contact) using E-beam evaporator. Photolithography using NR9-3000PY for thick metal stripe deposition 4. Spin HMDS (adhesion promoter) at 3000rpm for 40s. 5. Spin NR9-3000PY at 5000rpm for 45s (~2.4m photoresist thickness). 6. Bake at 150oC for 70s. 7. Expose with MA6 at 11mW/cm2 for 3~4s. 8. Bake at 100oC for 70s. 9. Develop in RD6 for 10s without agitation. Rinse with DI water. 165 166 10. Bake at 100oC for 70s. 11. Descum using O2 plasma in P80 and dip into HCl (1:3 diluted) for 30s. 12. Bake at 100oC for 70s. 13. Deposit thick metal (Cr/Au/Cr/Ni) using E-beam evaporator. 14. Lift off in acetone. Clean with IPA and DI water. Dry with N2 blow. Part II: Ni wet etch (Schottky gate patterning) Photolithography using S1818 for Ni wet etch 1. Spin HMDS at 3000rpm for 40s. 2. Spin S1818 at 5000rpm for 45s. 3. Bake at 115oC for 70s. 4. Expose with MA6 at 11mW/cm2 for 15s. 5. Develop in MF321 for 45s with agitation. Rinse with DI water. 6. Bake at 100oC for 70s. Ni wet etch 7. Immerse into HCl (1:1 diluted) for 1min. Rinse with DI water. 8. Immerse into Ni etchant until etched areas are clear. Rinse with DI water. 9. Remove photoresist and clean with acetone and IPA. Rinse with DI water. 167 Part III: GaN mesa etch 1. Sputter ~100nm SiO2. 2. Self-aligned etch SiO2 in P80 RIE etcher using Ar and CHF3 to form the sidewall protection layer for the thick Au. 3. Self-aligned etch ~1m GaN in P80 RIE etcher using BCl3/Cl2 at 0oC. 4. Remove GaN etch residuals in hot KOH solution (~90oC, 0.1mol/L) for 1min. Rinse with DI water. 5. Grow Al2O3 using ALD as GaN mesa sidewall protection layer at 170oC for ~70nm. 6. Self-aligned etch Al2O3 in P80 using Cl2/CHF3/Ar (only left Al2O3 on the GaN mesa sidewalls). Part IV: Ohmic contact deposition 1. Repeat the photolithography procedure from 4~12 in part I for ohmic metal deposition. 2. Deposit ohmic metal (Ti/Al/Ti/Au) using E-beam evaporator. 3. Lift off in acetone. Clean with IPA and DI water. Dry with N2 blow. Part V: Device isolation and the n+ GaN serpentine resistor 168 1. Repeat the photolithography procedure from 4~12 in part I for isolation pattern (as well as the serpentine resistor pattern). 2. Sputter ~150nm SiNx. 3. Deposit 200nm Ni using E-beam evaporator. 4. Lift off in acetone. Clean with IPA and DI water. Dry with N2 blow. 5. Etch ~ 2.8m GaN (n+ GaN and the GaN buffer layer) in P80 RIE etcher using BCl3/Cl2 at 0oC. 6. Remove GaN etch residuals in hot KOH solution (~90oC, 0.1mol/L) for 1min. Rinse with DI water. 7. Remove the Ni mask using HCl (1:1 diluted) followed by Ni etchant. Rinse with DI water after every wet etch. 8. Self-aligned etch the SiNx mask in P80 RIE etcher using CF4/O2. Part VI: BCB curing and etch 1. Spin AP3000 (adhesion promoter) at 3000rpm for 30s. 2. Bake at 125oC for 90s. 3. Dilute BCB with T1100 (optional). 4. Spin BCB at 500rpm for 10s, 1000rpm for 10s and 5000rpm for 45s. 5. Expose BCB using MA6 at 11mW/cm2 for 30s. 6. Develop in DS3000 at 35~40oC for 70s. 7. Stabilize in DS3000 at room temperature for 30s. 8. Spin dry at 2000rpm for 1min with N2 blow. 169 9. Bake at 90oC for 3min. 10. Soft cure in forming gas at 170oC for 15mins. Ramp up temperature slowly to avoid BCB cracking. 11. Second layer of BCB: repeat the procedure from 1 to 9 in part VI. 12. Second cure in forming gas at 170oC for 30mins. Ramp up temperature slowly to avoid BCB cracking. BCB etch 13. Repeat the photolithography procedure from 4~10 in part I for BCB etch mask. Baking time and develop time should be increased in this step. 14. Etch BCB in P80 RIE etcher using CF4/O2. 15. Remove the photoresist mask (NR9-3000PY) using acetone when it is etched to very thin. Clean with IPA and DI water. 16. Repeat the above steps 13~15 until the smallest vias are all clear. Part VII: Pad metal deposition 1. Repeat the photolithography procedure from 4~10 in part I for final pad metal deposition. Baking time and develop time should be increased in this step. 2. Descum in P80 RIE etcher using CF4/O2. 170 3. Immerse into Acetic acid (1:1 diluted) for 30s, HCl (1:3 diluted) for 30s and Ni etchant for 20s. Rinse with DI water after every wet etch. 4. Sputter Ti/Au (10nm/100nm) to improve the BCB sidewall coverage. 5. Deposit Au for 300nm using E-beam evaporator. 6. Lift off in acetone. Clean with IPA and DI water rinse. 7. To thicken the pad metal. Repeat the photolithography procedure from 4~12 in part I. Baking time and develop time should be increased in this step. 8. Deposit Ti/Au (10nm/700nm) using E-beam evaporator. 9. Lift off in acetone. Clean with IPA and DI water rinse.